# Electronic Supplementary Material (ESI) for CrystEngComm.
# This journal is © The Royal Society of Chemistry 2014

#######################################################################
#
#                 Cambridge Crystallographic Data Centre
#                                CCDC 
# 
#######################################################################
# 
#  This CIF contains data from an original supplementary publication
#  deposited with the CCDC, and may include chemical, crystal,
#  experimental, refinement, atomic coordinates,
#  anisotropic displacement parameters and molecular geometry data,
#  as required by the journal to which it was submitted.
#
#  This CIF is provided on the understanding that it is used for bona
#  fide research purposes only. It may contain copyright material
#  of the CCDC or of third parties, and may not be copied or further
#  disseminated in any form, whether machine-readable or not,
#  except for the purpose of generating routine backup copies
#  on your local computer system.
# 
#  For further information on the CCDC, data deposition and
#  data retrieval see:
#                         www.ccdc.cam.ac.uk
#
#  Bona fide researchers may freely download Mercury and enCIFer
#  from this site to visualise CIF-encoded structures and 
#  to carry out CIF format checking respectively.
#
data_2
#TrackingRef '2.txt'

_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'Cr4 Gd4 Mo24 O123.92, 16(O)'
_chemical_formula_sum            'Cr4 Gd4 Mo24 O139.92'
_chemical_formula_weight         5378.28

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cr Cr 0.3209 0.6236 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Gd Gd -0.1653 3.9035 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Orthorhombic
_symmetry_space_group_name_H-M   'P c a 21'
_symmetry_space_group_name_Hall  'P 2c -2ac'
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z+1/2'
'x+1/2, -y, z'
'-x+1/2, y, z+1/2'

_cell_length_a                   11.7941(17)
_cell_length_b                   10.9501(16)
_cell_length_c                   22.359(3)
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_volume                     2887.6(7)
_cell_formula_units_Z            1
_cell_measurement_temperature    298
_cell_measurement_reflns_used    8820
_cell_measurement_theta_min      2.25
_cell_measurement_theta_max      28.15

_exptl_crystal_description       block
_exptl_crystal_colour            pink
_exptl_crystal_size_max          0.45
_exptl_crystal_size_mid          0.30
_exptl_crystal_size_min          0.28
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    3.093
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             2479.2
_exptl_absorpt_coefficient_mu    5.266
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.294
_exptl_absorpt_correction_T_max  0.591
_exptl_absorpt_process_details   '(SADABS; Bruker, 2000)'

_exptl_special_details           
;
?
;

_diffrn_ambient_temperature      298
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            26204
_diffrn_reflns_av_R_equivalents  0.0405
_diffrn_reflns_av_sigmaI/netI    0.0330
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_l_min       -26
_diffrn_reflns_limit_l_max       26
_diffrn_reflns_theta_min         1.82
_diffrn_reflns_theta_max         25.00
_reflns_number_total             5150
_reflns_number_gt                5050
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
;
Refinement of F² against ALL reflections. The weighted R-factor wR and
goodness of fit S are based on F², conventional R-factors R are based
on F, with F set to zero for negative F². The threshold expression of
F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is
not relevant to the choice of reflections for refinement. R-factors based
on F² are statistically about twice as large as those based on F, and R-
factors based on ALL data will be even larger.
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0096P)²+14.4398P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   ...
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.140(11)
_refine_ls_number_reflns         5055
_refine_ls_number_parameters     390
_refine_ls_number_restraints     1
_refine_ls_R_factor_all          0.0286
_refine_ls_R_factor_gt           0.0284
_refine_ls_wR_factor_ref         0.0648
_refine_ls_wR_factor_gt          0.0647
_refine_ls_goodness_of_fit_ref   1.190
_refine_ls_restrained_S_all      1.190
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.00

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Gd1 Gd 0.17153(3) 0.25013(3) 1.00177(2) 0.01874(9) Uani 1 1 d . . .
Mo1 Mo 0.29536(6) 0.50443(6) 0.87932(3) 0.01607(16) Uani 1 1 d . . .
Mo2 Mo 0.19631(5) 0.75222(6) 0.94917(3) 0.01726(15) Uani 1 1 d . . .
Mo3 Mo 0.09806(6) 0.98859(6) 0.87214(3) 0.01631(15) Uani 1 1 d . . .
Mo4 Mo 0.09518(6) 0.97827(6) 0.72303(3) 0.01803(16) Uani 1 1 d . . .
Mo5 Mo 0.19641(6) 0.73511(6) 0.65255(3) 0.01807(15) Uani 1 1 d . . .
Mo6 Mo 0.29986(6) 0.50142(6) 0.73016(3) 0.01694(16) Uani 1 1 d . . .
Cr1 Cr 0.19804(9) 0.74475(9) 0.80123(6) 0.0132(2) Uani 1 1 d . . .
O1 O 0.2236(5) 0.4110(5) 0.9286(3) 0.0269(14) Uani 1 1 d . . .
O2 O 0.4323(5) 0.4510(5) 0.8780(3) 0.0245(13) Uani 1 1 d . . .
O3 O 0.3221(5) 0.6434(5) 0.9278(2) 0.0189(12) Uani 1 1 d . . .
O4 O 0.1254(5) 0.6622(5) 0.9994(3) 0.0292(13) Uani 1 1 d . . .
O5 O 0.2761(5) 0.8535(5) 0.9890(3) 0.0253(14) Uani 1 1 d . . .
O6 O 0.0716(5) 0.8522(5) 0.9241(2) 0.0182(12) Uani 1 1 d . . .
O7 O -0.0386(5) 1.0422(5) 0.8698(3) 0.0253(13) Uani 1 1 d . . .
O8 O 0.1679(5) 1.0851(5) 0.9202(3) 0.0240(13) Uani 1 1 d . . .
O9 O 0.1551(4) 1.0505(4) 0.7977(3) 0.0195(10) Uani 1 1 d . . .
O10 O -0.0370(5) 1.0374(6) 0.7263(3) 0.0344(15) Uani 1 1 d . . .
O11 O 0.1699(6) 1.0677(5) 0.6747(3) 0.0339(15) Uani 1 1 d . . .
O12 O 0.0685(5) 0.8353(5) 0.6745(3) 0.0202(12) Uani 1 1 d . . .
O13 O 0.2736(6) 0.8314(6) 0.6097(3) 0.0324(15) Uani 1 1 d . . .
O14 O 0.1306(6) 0.6371(6) 0.6049(3) 0.0332(15) Uani 1 1 d . . .
O15 O 0.3233(5) 0.6333(5) 0.6770(2) 0.0191(12) Uani 1 1 d . . .
O16 O 0.2285(5) 0.3983(5) 0.6871(3) 0.0285(14) Uani 1 1 d . . .
O17 O 0.4336(5) 0.4463(5) 0.7355(3) 0.0295(14) Uani 1 1 d . . .
O18 O 0.2380(4) 0.4390(4) 0.8060(3) 0.0180(10) Uani 1 1 d . . .
O19 O 0.1469(4) 0.6394(4) 0.8679(2) 0.0157(11) Uani 1 1 d . . .
O20 O 0.2489(5) 0.8557(5) 0.8643(2) 0.0146(11) Uani 1 1 d . . .
O21 O 0.0613(4) 0.8466(4) 0.7995(3) 0.0170(10) Uani 1 1 d . . .
O22 O 0.2474(4) 0.8494(5) 0.7351(2) 0.0168(12) Uani 1 1 d . . .
O23 O 0.1482(4) 0.6311(5) 0.7377(2) 0.0149(11) Uani 1 1 d . . .
O24 O 0.3342(3) 0.6398(4) 0.8025(3) 0.0146(10) Uani 1 1 d . . .
O25 O 0.0318(6) 0.2846(6) 0.9276(3) 0.0398(16) Uani 1 1 d . . .
O26 O 0.3571(6) 0.2095(7) 0.9620(4) 0.051(2) Uani 1 1 d . . .
O27 O 0.2465(7) 0.0704(5) 1.0488(3) 0.0322(13) Uani 1 1 d . . .
O28 O 0.0055(5) 0.1327(6) 1.0252(3) 0.0324(14) Uani 1 1 d . . .
O29 O 0.1345(5) 0.2442(5) 1.1121(3) 0.0328(14) Uani 1 1 d . . .
O30 O 0.0578(6) 0.4256(6) 1.0303(3) 0.050(2) Uani 1 1 d . . .
O1W O 0.5504(5) 0.7089(5) 0.8020(4) 0.0428(15) Uani 1 1 d . . .
O2W O 0.8456(5) 0.7973(6) 0.8175(4) 0.045(2) Uani 1 1 d . . .
O3W O 0.9685(7) 0.6839(11) 0.1278(5) 0.085(3) Uani 1 1 d . . .
O4W O 0.5088(9) 0.0950(8) 0.0675(4) 0.072(4) Uani 1.00(2) 1 d . . .
O31 O 0.3048(6) 0.3868(7) 1.0512(3) 0.049(2) Uani 0.98 1 d P . .


_geom_special_details            
;
All esds (except the esd in the dihedral angle between two l.s. planes)
are estimated using the full covariance matrix. The cell esds are taken
into account individually in the estimation of esds in distances, angles
and torsion angles; correlations between esds in cell parameters are only
used when they are defined by crystal symmetry. An approximate (isotropic)
treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Gd1 O25 2.369(6) . ?
Gd1 O27 2.400(6) . ?
Gd1 O28 2.401(6) . ?
Gd1 O26 2.404(6) . ?
Gd1 O30 2.428(6) . ?
Gd1 O31 2.436(6) . ?
Gd1 O1 2.481(6) . ?
Gd1 O29 2.506(6) . ?
Gd1 O8 2.567(6) 1_545 ?
Mo1 O2 1.718(5) . ?
Mo1 O1 1.725(6) . ?
Mo1 O3 1.895(6) . ?
Mo1 O18 1.912(6) . ?
Mo1 O19 2.305(5) . ?
Mo1 O24 2.314(5) . ?
Mo2 O5 1.706(6) . ?
Mo2 O4 1.712(6) . ?
Mo2 O6 1.917(6) . ?
Mo2 O3 1.962(6) . ?
Mo2 O19 2.274(5) . ?
Mo2 O20 2.295(5) . ?
Mo3 O7 1.716(6) . ?
Mo3 O8 1.718(6) . ?
Mo3 O6 1.918(6) . ?
Mo3 O9 1.920(6) . ?
Mo3 O21 2.290(6) . ?
Mo3 O20 2.305(5) . ?
Mo4 O10 1.689(6) . ?
Mo4 O11 1.704(6) . ?
Mo4 O12 1.931(5) . ?
Mo4 O9 1.977(6) . ?
Mo4 O21 2.272(6) . ?
Mo4 O22 2.300(5) . ?
Mo5 O13 1.691(6) . ?
Mo5 O14 1.699(6) . ?
Mo5 O12 1.928(6) . ?
Mo5 O15 1.944(6) . ?
Mo5 O23 2.291(5) . ?
Mo5 O22 2.310(5) . ?
Mo6 O17 1.693(6) . ?
Mo6 O16 1.706(6) . ?
Mo6 O15 1.891(5) . ?
Mo6 O18 1.969(6) . ?
Mo6 O24 2.254(5) . ?
Mo6 O23 2.290(5) . ?
Cr1 O20 1.956(5) . ?
Cr1 O22 1.959(5) . ?
Cr1 O21 1.961(4) . ?
Cr1 O24 1.975(4) . ?
Cr1 O23 1.977(5) . ?
Cr1 O19 1.979(5) . ?
O8 Gd1 2.567(6) 1_565 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O25 Gd1 O27 133.9(2) . . ?
O25 Gd1 O28 70.8(2) . . ?
O27 Gd1 O28 76.4(2) . . ?
O25 Gd1 O26 113.8(3) . . ?
O27 Gd1 O26 71.0(3) . . ?
O28 Gd1 O26 136.4(2) . . ?
O25 Gd1 O30 70.9(3) . . ?
O27 Gd1 O30 137.5(2) . . ?
O28 Gd1 O30 85.2(2) . . ?
O26 Gd1 O30 138.3(2) . . ?
O25 Gd1 O31 132.0(3) . . ?
O27 Gd1 O31 93.8(3) . . ?
O28 Gd1 O31 139.1(2) . . ?
O26 Gd1 O31 72.2(3) . . ?
O30 Gd1 O31 75.6(3) . . ?
O25 Gd1 O1 66.3(2) . . ?
O27 Gd1 O1 141.2(2) . . ?
O28 Gd1 O1 136.6(2) . . ?
O26 Gd1 O1 70.2(2) . . ?
O30 Gd1 O1 75.4(2) . . ?
O31 Gd1 O1 72.7(2) . . ?
O25 Gd1 O29 124.9(2) . . ?
O27 Gd1 O29 67.1(2) . . ?
O28 Gd1 O29 68.2(2) . . ?
O26 Gd1 O29 121.2(3) . . ?
O30 Gd1 O29 70.5(2) . . ?
O31 Gd1 O29 71.4(2) . . ?
O1 Gd1 O29 135.3(2) . . ?
O25 Gd1 O8 66.6(2) . 1_545 ?
O27 Gd1 O8 75.0(2) . 1_545 ?
O28 Gd1 O8 76.4(2) . 1_545 ?
O26 Gd1 O8 67.8(2) . 1_545 ?
O30 Gd1 O8 137.2(2) . 1_545 ?
O31 Gd1 O8 140.0(2) . 1_545 ?
O1 Gd1 O8 92.0(2) . 1_545 ?
O29 Gd1 O8 132.68(19) . 1_545 ?
O2 Mo1 O1 105.6(3) . . ?
O2 Mo1 O3 97.3(3) . . ?
O1 Mo1 O3 101.1(3) . . ?
O2 Mo1 O18 101.0(2) . . ?
O1 Mo1 O18 98.7(3) . . ?
O3 Mo1 O18 148.2(2) . . ?
O2 Mo1 O19 158.5(2) . . ?
O1 Mo1 O19 94.5(3) . . ?
O3 Mo1 O19 71.0(2) . . ?
O18 Mo1 O19 82.91(19) . . ?
O2 Mo1 O24 91.1(2) . . ?
O1 Mo1 O24 162.0(2) . . ?
O3 Mo1 O24 82.9(2) . . ?
O18 Mo1 O24 71.00(19) . . ?
O19 Mo1 O24 69.97(16) . . ?
O5 Mo2 O4 107.5(3) . . ?
O5 Mo2 O6 101.8(3) . . ?
O4 Mo2 O6 98.4(3) . . ?
O5 Mo2 O3 96.0(3) . . ?
O4 Mo2 O3 100.3(3) . . ?
O6 Mo2 O3 148.9(2) . . ?
O5 Mo2 O19 155.8(2) . . ?
O4 Mo2 O19 94.9(3) . . ?
O6 Mo2 O19 83.1(2) . . ?
O3 Mo2 O19 70.7(2) . . ?
O5 Mo2 O20 87.8(2) . . ?
O4 Mo2 O20 163.4(3) . . ?
O6 Mo2 O20 71.6(2) . . ?
O3 Mo2 O20 83.9(2) . . ?
O19 Mo2 O20 71.14(19) . . ?
O7 Mo3 O8 105.0(3) . . ?
O7 Mo3 O6 97.6(3) . . ?
O8 Mo3 O6 100.2(3) . . ?
O7 Mo3 O9 100.4(3) . . ?
O8 Mo3 O9 99.1(3) . . ?
O6 Mo3 O9 149.1(2) . . ?
O7 Mo3 O21 91.9(2) . . ?
O8 Mo3 O21 162.2(2) . . ?
O6 Mo3 O21 82.6(2) . . ?
O9 Mo3 O21 71.99(19) . . ?
O7 Mo3 O20 159.8(2) . . ?
O8 Mo3 O20 93.8(2) . . ?
O6 Mo3 O20 71.3(2) . . ?
O9 Mo3 O20 83.52(19) . . ?
O21 Mo3 O20 70.34(16) . . ?
O10 Mo4 O11 106.5(3) . . ?
O10 Mo4 O12 100.7(3) . . ?
O11 Mo4 O12 101.2(3) . . ?
O10 Mo4 O9 98.0(3) . . ?
O11 Mo4 O9 96.9(3) . . ?
O12 Mo4 O9 149.0(2) . . ?
O10 Mo4 O21 92.8(3) . . ?
O11 Mo4 O21 158.9(3) . . ?
O12 Mo4 O21 83.1(2) . . ?
O9 Mo4 O21 71.5(2) . . ?
O10 Mo4 O22 161.9(3) . . ?
O11 Mo4 O22 91.4(3) . . ?
O12 Mo4 O22 72.3(2) . . ?
O9 Mo4 O22 82.37(19) . . ?
O21 Mo4 O22 70.07(17) . . ?
O13 Mo5 O14 106.6(3) . . ?
O13 Mo5 O12 102.1(3) . . ?
O14 Mo5 O12 99.3(3) . . ?
O13 Mo5 O15 95.9(3) . . ?
O14 Mo5 O15 99.5(3) . . ?
O12 Mo5 O15 149.0(3) . . ?
O13 Mo5 O23 156.2(3) . . ?
O14 Mo5 O23 95.4(3) . . ?
O12 Mo5 O23 83.0(2) . . ?
O15 Mo5 O23 70.9(2) . . ?
O13 Mo5 O22 88.5(3) . . ?
O14 Mo5 O22 164.1(3) . . ?
O12 Mo5 O22 72.1(2) . . ?
O15 Mo5 O22 83.4(2) . . ?
O23 Mo5 O22 70.69(19) . . ?
O17 Mo6 O16 105.3(3) . . ?
O17 Mo6 O15 100.4(3) . . ?
O16 Mo6 O15 102.9(3) . . ?
O17 Mo6 O18 99.2(2) . . ?
O16 Mo6 O18 94.2(3) . . ?
O15 Mo6 O18 149.4(2) . . ?
O17 Mo6 O24 91.2(2) . . ?
O16 Mo6 O24 159.9(2) . . ?
O15 Mo6 O24 84.9(2) . . ?
O18 Mo6 O24 71.44(19) . . ?
O17 Mo6 O23 160.6(2) . . ?
O16 Mo6 O23 93.9(2) . . ?
O15 Mo6 O23 71.8(2) . . ?
O18 Mo6 O23 82.08(18) . . ?
O24 Mo6 O23 70.75(16) . . ?
O20 Cr1 O22 95.15(19) . . ?
O20 Cr1 O21 85.1(2) . . ?
O22 Cr1 O21 84.1(2) . . ?
O20 Cr1 O24 95.8(2) . . ?
O22 Cr1 O24 96.3(2) . . ?
O21 Cr1 O24 179.0(2) . . ?
O20 Cr1 O23 179.2(2) . . ?
O22 Cr1 O23 85.1(2) . . ?
O21 Cr1 O23 95.7(2) . . ?
O24 Cr1 O23 83.5(2) . . ?
O20 Cr1 O19 85.0(2) . . ?
O22 Cr1 O19 179.6(2) . . ?
O21 Cr1 O19 95.5(2) . . ?
O24 Cr1 O19 84.1(2) . . ?
O23 Cr1 O19 94.78(19) . . ?
Mo1 O1 Gd1 164.5(4) . . ?
Mo1 O3 Mo2 120.1(3) . . ?
Mo2 O6 Mo3 119.8(3) . . ?
Mo3 O8 Gd1 152.3(3) . 1_565 ?
Mo3 O9 Mo4 117.7(2) . . ?
Mo5 O12 Mo4 118.5(3) . . ?
Mo6 O15 Mo5 120.1(3) . . ?
Mo1 O18 Mo6 118.5(2) . . ?
Cr1 O19 Mo2 102.0(2) . . ?
Cr1 O19 Mo1 103.1(2) . . ?
Mo2 O19 Mo1 93.7(2) . . ?
Cr1 O20 Mo2 101.9(2) . . ?
Cr1 O20 Mo3 102.1(2) . . ?
Mo2 O20 Mo3 92.31(19) . . ?
Cr1 O21 Mo4 103.4(2) . . ?
Cr1 O21 Mo3 102.5(2) . . ?
Mo4 O21 Mo3 93.98(16) . . ?
Cr1 O22 Mo4 102.4(2) . . ?
Cr1 O22 Mo5 102.0(2) . . ?
Mo4 O22 Mo5 92.00(18) . . ?
Cr1 O23 Mo6 102.2(2) . . ?
Cr1 O23 Mo5 102.2(2) . . ?
Mo6 O23 Mo5 93.03(18) . . ?
Cr1 O24 Mo6 103.6(2) . . ?
Cr1 O24 Mo1 102.9(2) . . ?
Mo6 O24 Mo1 93.80(16) . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O2 Mo1 O1 Gd1 0.0(13) . . . . ?
O3 Mo1 O1 Gd1 -100.9(13) . . . . ?
O18 Mo1 O1 Gd1 104.1(12) . . . . ?
O19 Mo1 O1 Gd1 -172.4(12) . . . . ?
O24 Mo1 O1 Gd1 157.8(8) . . . . ?
O25 Gd1 O1 Mo1 -139.7(13) . . . . ?
O27 Gd1 O1 Mo1 -8.1(14) . . . . ?
O28 Gd1 O1 Mo1 -148.6(12) . . . . ?
O26 Gd1 O1 Mo1 -10.9(12) . . . . ?
O30 Gd1 O1 Mo1 145.1(13) . . . . ?
O31 Gd1 O1 Mo1 65.9(13) . . . . ?
O29 Gd1 O1 Mo1 104.0(13) . . . . ?
O8 Gd1 O1 Mo1 -76.4(13) 1_545 . . . ?
O2 Mo1 O3 Mo2 -179.6(3) . . . . ?
O1 Mo1 O3 Mo2 -72.0(4) . . . . ?
O18 Mo1 O3 Mo2 55.6(6) . . . . ?
O19 Mo1 O3 Mo2 19.0(3) . . . . ?
O24 Mo1 O3 Mo2 90.2(3) . . . . ?
O5 Mo2 O3 Mo1 -178.6(3) . . . . ?
O4 Mo2 O3 Mo1 72.3(4) . . . . ?
O6 Mo2 O3 Mo1 -53.7(6) . . . . ?
O19 Mo2 O3 Mo1 -19.3(3) . . . . ?
O20 Mo2 O3 Mo1 -91.4(3) . . . . ?
O5 Mo2 O6 Mo3 63.4(4) . . . . ?
O4 Mo2 O6 Mo3 173.4(3) . . . . ?
O3 Mo2 O6 Mo3 -60.2(6) . . . . ?
O19 Mo2 O6 Mo3 -92.6(3) . . . . ?
O20 Mo2 O6 Mo3 -20.3(3) . . . . ?
O7 Mo3 O6 Mo2 -177.2(3) . . . . ?
O8 Mo3 O6 Mo2 -70.3(4) . . . . ?
O9 Mo3 O6 Mo2 57.5(6) . . . . ?
O21 Mo3 O6 Mo2 91.9(3) . . . . ?
O20 Mo3 O6 Mo2 20.2(3) . . . . ?
O7 Mo3 O8 Gd1 15.5(7) . . . 1_565 ?
O6 Mo3 O8 Gd1 -85.3(7) . . . 1_565 ?
O9 Mo3 O8 Gd1 119.0(7) . . . 1_565 ?
O21 Mo3 O8 Gd1 177.1(5) . . . 1_565 ?
O20 Mo3 O8 Gd1 -157.0(6) . . . 1_565 ?
O7 Mo3 O9 Mo4 -69.2(3) . . . . ?
O8 Mo3 O9 Mo4 -176.4(3) . . . . ?
O6 Mo3 O9 Mo4 55.5(5) . . . . ?
O21 Mo3 O9 Mo4 19.4(2) . . . . ?
O20 Mo3 O9 Mo4 90.8(3) . . . . ?
O10 Mo4 O9 Mo3 70.6(3) . . . . ?
O11 Mo4 O9 Mo3 178.5(3) . . . . ?
O12 Mo4 O9 Mo3 -56.0(5) . . . . ?
O21 Mo4 O9 Mo3 -19.6(2) . . . . ?
O22 Mo4 O9 Mo3 -91.1(3) . . . . ?
O13 Mo5 O12 Mo4 -64.1(4) . . . . ?
O14 Mo5 O12 Mo4 -173.4(3) . . . . ?
O15 Mo5 O12 Mo4 60.0(6) . . . . ?
O23 Mo5 O12 Mo4 92.2(3) . . . . ?
O22 Mo5 O12 Mo4 20.3(3) . . . . ?
O10 Mo4 O12 Mo5 176.9(4) . . . . ?
O11 Mo4 O12 Mo5 67.5(4) . . . . ?
O9 Mo4 O12 Mo5 -57.1(6) . . . . ?
O21 Mo4 O12 Mo5 -91.6(3) . . . . ?
O22 Mo4 O12 Mo5 -20.4(3) . . . . ?
O17 Mo6 O15 Mo5 179.7(3) . . . . ?
O16 Mo6 O15 Mo5 71.3(4) . . . . ?
O18 Mo6 O15 Mo5 -51.1(6) . . . . ?
O24 Mo6 O15 Mo5 -89.9(3) . . . . ?
O23 Mo6 O15 Mo5 -18.5(3) . . . . ?
O13 Mo5 O15 Mo6 178.3(3) . . . . ?
O14 Mo5 O15 Mo6 -73.8(4) . . . . ?
O12 Mo5 O15 Mo6 52.8(6) . . . . ?
O23 Mo5 O15 Mo6 18.6(3) . . . . ?
O22 Mo5 O15 Mo6 90.4(3) . . . . ?
O2 Mo1 O18 Mo6 -67.1(3) . . . . ?
O1 Mo1 O18 Mo6 -175.1(3) . . . . ?
O3 Mo1 O18 Mo6 56.9(5) . . . . ?
O19 Mo1 O18 Mo6 91.5(3) . . . . ?
O24 Mo1 O18 Mo6 20.3(2) . . . . ?
O17 Mo6 O18 Mo1 67.4(3) . . . . ?
O16 Mo6 O18 Mo1 173.6(3) . . . . ?
O15 Mo6 O18 Mo1 -62.0(5) . . . . ?
O24 Mo6 O18 Mo1 -20.8(2) . . . . ?
O23 Mo6 O18 Mo1 -93.0(3) . . . . ?
O20 Cr1 O19 Mo2 0.5(2) . . . . ?
O21 Cr1 O19 Mo2 -84.0(2) . . . . ?
O24 Cr1 O19 Mo2 96.9(2) . . . . ?
O23 Cr1 O19 Mo2 179.8(2) . . . . ?
O20 Cr1 O19 Mo1 -96.2(2) . . . . ?
O22 Cr1 O19 Mo1 159(88) . . . . ?
O21 Cr1 O19 Mo1 179.3(2) . . . . ?
O24 Cr1 O19 Mo1 0.2(2) . . . . ?
O23 Cr1 O19 Mo1 83.1(2) . . . . ?
O5 Mo2 O19 Cr1 -31.2(6) . . . . ?
O4 Mo2 O19 Cr1 170.2(3) . . . . ?
O6 Mo2 O19 Cr1 72.4(3) . . . . ?
O3 Mo2 O19 Cr1 -90.6(3) . . . . ?
O20 Mo2 O19 Cr1 -0.49(18) . . . . ?
O5 Mo2 O19 Mo1 73.0(6) . . . . ?
O4 Mo2 O19 Mo1 -85.6(2) . . . . ?
O6 Mo2 O19 Mo1 176.6(2) . . . . ?
O3 Mo2 O19 Mo1 13.6(2) . . . . ?
O20 Mo2 O19 Mo1 103.7(2) . . . . ?
O2 Mo1 O19 Cr1 29.6(8) . . . . ?
O1 Mo1 O19 Cr1 -170.7(3) . . . . ?
O3 Mo1 O19 Cr1 89.1(3) . . . . ?
O18 Mo1 O19 Cr1 -72.5(2) . . . . ?
O24 Mo1 O19 Cr1 -0.2(2) . . . . ?
O2 Mo1 O19 Mo2 -73.6(7) . . . . ?
O1 Mo1 O19 Mo2 86.1(2) . . . . ?
O3 Mo1 O19 Mo2 -14.1(2) . . . . ?
O18 Mo1 O19 Mo2 -175.7(2) . . . . ?
O24 Mo1 O19 Mo2 -103.4(2) . . . . ?
O22 Cr1 O20 Mo2 179.0(3) . . . . ?
O21 Cr1 O20 Mo2 95.5(2) . . . . ?
O24 Cr1 O20 Mo2 -84.1(2) . . . . ?
O19 Cr1 O20 Mo2 -0.5(2) . . . . ?
O22 Cr1 O20 Mo3 84.0(2) . . . . ?
O21 Cr1 O20 Mo3 0.4(2) . . . . ?
O24 Cr1 O20 Mo3 -179.1(2) . . . . ?
O23 Cr1 O20 Mo3 -166(88) . . . . ?
O19 Cr1 O20 Mo3 -95.6(2) . . . . ?
O5 Mo2 O20 Cr1 168.4(3) . . . . ?
O4 Mo2 O20 Cr1 -33.8(9) . . . . ?
O6 Mo2 O20 Cr1 -88.4(3) . . . . ?
O3 Mo2 O20 Cr1 72.1(2) . . . . ?
O19 Mo2 O20 Cr1 0.50(18) . . . . ?
O5 Mo2 O20 Mo3 -88.7(2) . . . . ?
O4 Mo2 O20 Mo3 69.1(8) . . . . ?
O6 Mo2 O20 Mo3 14.49(19) . . . . ?
O3 Mo2 O20 Mo3 175.0(2) . . . . ?
O19 Mo2 O20 Mo3 103.4(2) . . . . ?
O7 Mo3 O20 Cr1 29.1(8) . . . . ?
O8 Mo3 O20 Cr1 -172.2(3) . . . . ?
O6 Mo3 O20 Cr1 88.2(3) . . . . ?
O9 Mo3 O20 Cr1 -73.5(2) . . . . ?
O21 Mo3 O20 Cr1 -0.4(2) . . . . ?
O7 Mo3 O20 Mo2 -73.6(7) . . . . ?
O8 Mo3 O20 Mo2 85.0(2) . . . . ?
O6 Mo3 O20 Mo2 -14.51(19) . . . . ?
O9 Mo3 O20 Mo2 -176.3(2) . . . . ?
O21 Mo3 O20 Mo2 -103.1(2) . . . . ?
O20 Cr1 O21 Mo4 96.8(2) . . . . ?
O22 Cr1 O21 Mo4 1.1(2) . . . . ?
O23 Cr1 O21 Mo4 -83.4(2) . . . . ?
O19 Cr1 O21 Mo4 -178.8(2) . . . . ?
O20 Cr1 O21 Mo3 -0.4(2) . . . . ?
O22 Cr1 O21 Mo3 -96.1(2) . . . . ?
O23 Cr1 O21 Mo3 179.4(2) . . . . ?
O19 Cr1 O21 Mo3 84.0(2) . . . . ?
O10 Mo4 O21 Cr1 173.1(3) . . . . ?
O11 Mo4 O21 Cr1 -30.5(8) . . . . ?
O12 Mo4 O21 Cr1 72.7(3) . . . . ?
O9 Mo4 O21 Cr1 -89.4(2) . . . . ?
O22 Mo4 O21 Cr1 -1.0(2) . . . . ?
O10 Mo4 O21 Mo3 -83.1(3) . . . . ?
O11 Mo4 O21 Mo3 73.3(7) . . . . ?
O12 Mo4 O21 Mo3 176.5(2) . . . . ?
O9 Mo4 O21 Mo3 14.44(16) . . . . ?
O22 Mo4 O21 Mo3 102.88(19) . . . . ?
O7 Mo3 O21 Cr1 -169.8(3) . . . . ?
O8 Mo3 O21 Cr1 28.0(9) . . . . ?
O6 Mo3 O21 Cr1 -72.4(3) . . . . ?
O9 Mo3 O21 Cr1 89.8(2) . . . . ?
O20 Mo3 O21 Cr1 0.4(2) . . . . ?
O7 Mo3 O21 Mo4 85.5(2) . . . . ?
O8 Mo3 O21 Mo4 -76.7(8) . . . . ?
O6 Mo3 O21 Mo4 -177.0(2) . . . . ?
O9 Mo3 O21 Mo4 -14.84(17) . . . . ?
O20 Mo3 O21 Mo4 -104.27(19) . . . . ?
O20 Cr1 O22 Mo4 -85.5(2) . . . . ?
O21 Cr1 O22 Mo4 -1.1(2) . . . . ?
O24 Cr1 O22 Mo4 178.0(2) . . . . ?
O23 Cr1 O22 Mo4 95.2(2) . . . . ?
O20 Cr1 O22 Mo5 179.7(3) . . . . ?
O21 Cr1 O22 Mo5 -95.9(2) . . . . ?
O24 Cr1 O22 Mo5 83.2(2) . . . . ?
O23 Cr1 O22 Mo5 0.38(19) . . . . ?
O10 Mo4 O22 Cr1 -18.5(9) . . . . ?
O11 Mo4 O22 Cr1 170.7(3) . . . . ?
O12 Mo4 O22 Cr1 -88.0(3) . . . . ?
O9 Mo4 O22 Cr1 73.9(2) . . . . ?
O21 Mo4 O22 Cr1 1.0(2) . . . . ?
O10 Mo4 O22 Mo5 84.3(9) . . . . ?
O11 Mo4 O22 Mo5 -86.5(3) . . . . ?
O12 Mo4 O22 Mo5 14.8(2) . . . . ?
O9 Mo4 O22 Mo5 176.7(2) . . . . ?
O21 Mo4 O22 Mo5 103.8(2) . . . . ?
O13 Mo5 O22 Cr1 -168.4(3) . . . . ?
O14 Mo5 O22 Cr1 29.4(10) . . . . ?
O12 Mo5 O22 Cr1 88.3(3) . . . . ?
O15 Mo5 O22 Cr1 -72.4(2) . . . . ?
O23 Mo5 O22 Cr1 -0.35(18) . . . . ?
O13 Mo5 O22 Mo4 88.4(3) . . . . ?
O14 Mo5 O22 Mo4 -73.8(9) . . . . ?
O12 Mo5 O22 Mo4 -14.9(2) . . . . ?
O15 Mo5 O22 Mo4 -175.5(2) . . . . ?
O23 Mo5 O22 Mo4 -103.5(2) . . . . ?
O22 Cr1 O23 Mo6 95.5(2) . . . . ?
O21 Cr1 O23 Mo6 179.0(2) . . . . ?
O24 Cr1 O23 Mo6 -1.5(2) . . . . ?
O19 Cr1 O23 Mo6 -85.0(2) . . . . ?
O22 Cr1 O23 Mo5 -0.4(2) . . . . ?
O21 Cr1 O23 Mo5 83.2(2) . . . . ?
O24 Cr1 O23 Mo5 -97.3(2) . . . . ?
O19 Cr1 O23 Mo5 179.2(2) . . . . ?
O17 Mo6 O23 Cr1 -20.9(8) . . . . ?
O16 Mo6 O23 Cr1 168.1(3) . . . . ?
O15 Mo6 O23 Cr1 -89.6(3) . . . . ?
O18 Mo6 O23 Cr1 74.4(2) . . . . ?
O24 Mo6 O23 Cr1 1.34(19) . . . . ?
O17 Mo6 O23 Mo5 82.2(7) . . . . ?
O16 Mo6 O23 Mo5 -88.8(3) . . . . ?
O15 Mo6 O23 Mo5 13.5(2) . . . . ?
O18 Mo6 O23 Mo5 177.5(2) . . . . ?
O24 Mo6 O23 Mo5 104.5(2) . . . . ?
O13 Mo5 O23 Cr1 31.1(7) . . . . ?
O14 Mo5 O23 Cr1 -171.8(3) . . . . ?
O12 Mo5 O23 Cr1 -73.1(2) . . . . ?
O15 Mo5 O23 Cr1 90.0(3) . . . . ?
O22 Mo5 O23 Cr1 0.35(18) . . . . ?
O13 Mo5 O23 Mo6 -72.1(6) . . . . ?
O14 Mo5 O23 Mo6 85.0(3) . . . . ?
O12 Mo5 O23 Mo6 -176.3(2) . . . . ?
O15 Mo5 O23 Mo6 -13.2(2) . . . . ?
O22 Mo5 O23 Mo6 -102.8(2) . . . . ?
O20 Cr1 O24 Mo6 -178.7(2) . . . . ?
O22 Cr1 O24 Mo6 -82.8(2) . . . . ?
O23 Cr1 O24 Mo6 1.5(2) . . . . ?
O19 Cr1 O24 Mo6 97.0(2) . . . . ?
O20 Cr1 O24 Mo1 84.1(2) . . . . ?
O22 Cr1 O24 Mo1 180.0(2) . . . . ?
O23 Cr1 O24 Mo1 -95.7(2) . . . . ?
O19 Cr1 O24 Mo1 -0.2(2) . . . . ?
O17 Mo6 O24 Cr1 171.4(3) . . . . ?
O16 Mo6 O24 Cr1 -43.0(8) . . . . ?
O15 Mo6 O24 Cr1 71.1(2) . . . . ?
O18 Mo6 O24 Cr1 -89.2(2) . . . . ?
O23 Mo6 O24 Cr1 -1.35(19) . . . . ?
O17 Mo6 O24 Mo1 -84.4(2) . . . . ?
O16 Mo6 O24 Mo1 61.2(7) . . . . ?
O15 Mo6 O24 Mo1 175.3(2) . . . . ?
O18 Mo6 O24 Mo1 14.96(16) . . . . ?
O23 Mo6 O24 Mo1 102.86(18) . . . . ?
O2 Mo1 O24 Cr1 -169.4(3) . . . . ?
O1 Mo1 O24 Cr1 32.0(9) . . . . ?
O3 Mo1 O24 Cr1 -72.2(3) . . . . ?
O18 Mo1 O24 Cr1 89.4(2) . . . . ?
O19 Mo1 O24 Cr1 0.2(2) . . . . ?
O2 Mo1 O24 Mo6 85.8(2) . . . . ?
O1 Mo1 O24 Mo6 -72.9(8) . . . . ?
O3 Mo1 O24 Mo6 -177.0(2) . . . . ?
O18 Mo1 O24 Mo6 -15.46(16) . . . . ?
O19 Mo1 O24 Mo6 -104.69(19) . . . . ?

_diffrn_measured_fraction_theta_max 1.000
_diffrn_reflns_theta_full        25.00
_diffrn_measured_fraction_theta_full 1.000
_refine_diff_density_max         0.695
_refine_diff_density_min         -0.741
_refine_diff_density_rms         0.139


_database_code_depnum_ccdc_archive 'CCDC 922305'
#######################################################################
#
#                 Cambridge Crystallographic Data Centre
#                                CCDC 
# 
#######################################################################
# 
#  This CIF contains data from an original supplementary publication
#  deposited with the CCDC, and may include chemical, crystal,
#  experimental, refinement, atomic coordinates,
#  anisotropic displacement parameters and molecular geometry data,
#  as required by the journal to which it was submitted.
#
#  This CIF is provided on the understanding that it is used for bona
#  fide research purposes only. It may contain copyright material
#  of the CCDC or of third parties, and may not be copied or further
#  disseminated in any form, whether machine-readable or not,
#  except for the purpose of generating routine backup copies
#  on your local computer system.
# 
#  For further information on the CCDC, data deposition and
#  data retrieval see:
#                         www.ccdc.cam.ac.uk
#
#  Bona fide researchers may freely download Mercury and enCIFer
#  from this site to visualise CIF-encoded structures and 
#  to carry out CIF format checking respectively.
#
data_3

_audit_creation_method           'SHELXTL-NT2000 ver.6.12'
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'C6 H5 Cr Gd Mo6 N O30, C6 H5 N O2, 4(O)'
_chemical_formula_sum            'C12 H10 Cr Gd Mo6 N2 O36'
_chemical_formula_weight         1543.11

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cr Cr 0.3209 0.6236 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Gd Gd -0.1653 3.9035 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Monoclinic
_symmetry_space_group_name_H-M   C2/c
_symmetry_space_group_name_Hall  '-C 2yc'
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'

_cell_length_a                   23.459(7)
_cell_length_b                   13.337(4)
_cell_length_c                   24.725(8)
_cell_angle_alpha                90.00
_cell_angle_beta                 102.957(5)
_cell_angle_gamma                90.00
_cell_volume                     7539(4)
_cell_formula_units_Z            8
_cell_measurement_temperature    298(2)
_cell_measurement_reflns_used    8819
_cell_measurement_theta_min      2.30
_cell_measurement_theta_max      28.28

_exptl_crystal_description       Block
_exptl_crystal_colour            Pink
_exptl_crystal_size_max          0.30
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.10
_exptl_crystal_density_meas      2.710
_exptl_crystal_density_diffrn    2.719
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             5792.0
_exptl_absorpt_coefficient_mu    4.057
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.043
_exptl_absorpt_correction_T_max  0.233
_exptl_absorpt_process_details   '(SADABS; Bruker, 2000)'

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      298(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            35202
_diffrn_reflns_av_R_equivalents  0.0520
_diffrn_reflns_av_sigmaI/netI    0.0380
_diffrn_reflns_limit_h_min       -27
_diffrn_reflns_limit_h_max       27
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_l_min       -29
_diffrn_reflns_limit_l_max       29
_diffrn_reflns_theta_min         1.69
_diffrn_reflns_theta_max         25.00
_reflns_number_total             6637
_reflns_number_gt                6325
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0273P)²+227.4976P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         6628
_refine_ls_number_parameters     524
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0678
_refine_ls_R_factor_gt           0.0635
_refine_ls_wR_factor_ref         0.1202
_refine_ls_wR_factor_gt          0.1183
_refine_ls_goodness_of_fit_ref   1.322
_refine_ls_restrained_S_all      1.322
_refine_ls_shift/su_max          0.00
_refine_ls_shift/su_mean         0.00

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
C1 C 0.5188(5) 0.7549(11) 0.9808(5) 0.038(3) Uani 1 1 d . . .
H1 H 0.5077 0.6978 0.9975 0.046 Uiso 1 1 calc R . .
C2 C 0.5158(5) 0.7560(9) 0.9245(5) 0.032(3) Uani 1 1 d . . .
H2 H 0.5014 0.7010 0.9025 0.038 Uiso 1 1 calc R . .
C3 C 0.5349(4) 0.8405(9) 0.9015(4) 0.025(3) Uani 1 1 d . . .
C4 C 0.5546(6) 0.9220(10) 0.9337(5) 0.036(3) Uani 1 1 d . . .
H4 H 0.5669 0.9794 0.9183 0.043 Uiso 1 1 calc R . .
C5 C 0.5558(6) 0.9171(11) 0.9897(5) 0.042(3) Uani 1 1 d . . .
H5 H 0.5696 0.9712 1.0127 0.050 Uiso 1 1 calc R . .
C6 C 0.5381(5) 0.8377(7) 0.8412(4) 0.019(2) Uani 1 1 d . . .
C7 C 0.9000(5) 0.0207(11) 0.4320(5) 0.038(3) Uani 1 1 d . . .
H7 H 0.9292 -0.0198 0.4527 0.046 Uiso 1 1 calc R . .
C8 C 0.8888(6) 0.0180(11) 0.3749(5) 0.042(3) Uani 1 1 d . . .
H8 H 0.9107 -0.0229 0.3568 0.051 Uiso 1 1 calc R . .
C9 C 0.8446(5) 0.0769(9) 0.3451(4) 0.026(2) Uani 1 1 d . . .
C10 C 0.8138(6) 0.1394(9) 0.3735(5) 0.033(3) Uani 1 1 d . . .
H10 H 0.7849 0.1816 0.3539 0.039 Uiso 1 1 calc R . .
C11 C 0.8266(5) 0.1385(9) 0.4310(5) 0.029(3) Uani 1 1 d . . .
H11 H 0.8051 0.1780 0.4503 0.034 Uiso 1 1 calc R . .
C12 C 0.8289(5) 0.0745(8) 0.2824(4) 0.027(3) Uani 1 1 d . . .
Cr1 Cr 0.78929(7) 0.88844(12) 0.60451(6) 0.0149(3) Uani 1 1 d . . .
Gd1 Gd 0.59326(2) 0.78822(4) 0.75027(2) 0.01538(13) Uani 1 1 d . . .
Mo1 Mo 0.65583(4) 0.81062(6) 0.61011(3) 0.0156(2) Uani 1 1 d . . .
Mo2 Mo 0.75698(4) 0.64567(7) 0.59680(4) 0.0186(2) Uani 1 1 d . . .
Mo3 Mo 0.89053(4) 0.71711(7) 0.59438(4) 0.0231(2) Uani 1 1 d . . .
Mo4 Mo 0.92602(4) 0.95938(7) 0.60524(4) 0.0200(2) Uani 1 1 d . . .
Mo5 Mo 0.82285(4) 1.12987(6) 0.61177(3) 0.0162(2) Uani 1 1 d . . .
Mo6 Mo 0.68928(4) 1.05305(7) 0.62086(4) 0.0194(2) Uani 1 1 d . . .
N1 N 0.5371(5) 0.8342(10) 1.0107(4) 0.047(3) Uani 1 1 d . . .
H1B H 0.5371 0.8330 1.0455 0.057 Uiso 1 1 calc R . .
N2 N 0.8691(4) 0.0815(7) 0.4580(4) 0.026(2) Uani 1 1 d . . .
H1A H 0.8775 0.0831 0.4937 0.031 Uiso 1 1 calc R . .
O1 O 0.6217(3) 0.8168(6) 0.6652(3) 0.0251(17) Uani 1 1 d . . .
O2 O 0.6102(3) 0.7432(6) 0.5614(3) 0.0274(18) Uani 1 1 d . . .
O3 O 0.7091(3) 0.7038(5) 0.6424(3) 0.0223(16) Uani 1 1 d . . .
O4 O 0.7055(3) 0.5933(6) 0.5449(3) 0.0288(18) Uani 1 1 d . . .
O5 O 0.7878(4) 0.5485(6) 0.6382(3) 0.0334(19) Uani 1 1 d . . .
O6 O 0.8159(3) 0.6653(5) 0.5537(3) 0.0218(16) Uani 1 1 d . . .
O7 O 0.9137(4) 0.6258(6) 0.6423(4) 0.037(2) Uani 1 1 d . . .
O8 O 0.9300(3) 0.6977(7) 0.5457(3) 0.040(2) Uani 1 1 d . . .
O9 O 0.9344(3) 0.8284(6) 0.6360(3) 0.0267(17) Uani 1 1 d . . .
O10 O 0.9612(3) 0.9504(6) 0.5518(3) 0.0301(18) Uani 1 1 d . . .
O11 O 0.9724(3) 1.0232(6) 0.6567(3) 0.035(2) Uani 1 1 d . . .
O12 O 0.8742(3) 1.0703(5) 0.5702(3) 0.0174(15) Uani 1 1 d . . .
O13 O 0.8713(3) 1.1928(6) 0.6633(3) 0.0246(17) Uani 1 1 d . . .
O14 O 0.7928(3) 1.2184(6) 0.5642(3) 0.0308(18) Uani 1 1 d . . .
O15 O 0.7635(3) 1.1158(5) 0.6546(3) 0.0187(15) Uani 1 1 d . . .
O16 O 0.6597(3) 1.1436(6) 0.5753(4) 0.036(2) Uani 1 1 d . . .
O17 O 0.6562(4) 1.0652(6) 0.6751(3) 0.036(2) Uani 1 1 d . . .
O18 O 0.6448(3) 0.9427(5) 0.5806(3) 0.0174(15) Uani 1 1 d . . .
O19 O 0.7263(3) 0.8033(5) 0.5611(3) 0.0158(14) Uani 1 1 d . . .
O20 O 0.8207(3) 0.7621(5) 0.6412(3) 0.0185(15) Uani 1 1 d . . .
O21 O 0.8482(3) 0.8646(5) 0.5596(3) 0.0183(15) Uani 1 1 d . . .
O22 O 0.8508(3) 0.9753(5) 0.6485(3) 0.0152(14) Uani 1 1 d . . .
O23 O 0.7572(3) 1.0144(5) 0.5688(3) 0.0166(15) Uani 1 1 d . . .
O24 O 0.7345(3) 0.9100(5) 0.6526(3) 0.0147(14) Uani 1 1 d . . .
O25 O 0.5619(3) 0.6215(6) 0.7278(3) 0.0335(19) Uani 1 1 d . . .
O26 O 0.6801(3) 0.6896(6) 0.7449(3) 0.0290(18) Uani 1 1 d . . .
O27 O 0.6770(4) 0.8876(6) 0.7898(3) 0.036(2) Uani 1 1 d . . .
O28 O 0.5659(4) 0.9557(6) 0.7129(4) 0.036(2) Uani 1 1 d . . .
O29 O 0.5769(4) 0.8901(6) 0.8276(3) 0.0316(19) Uani 1 1 d . . .
O30 O 0.5059(3) 0.7798(6) 0.8079(3) 0.0297(18) Uani 1 1 d . . .
O31 O 0.8672(4) 0.0416(6) 0.2585(3) 0.0325(19) Uani 1 1 d . . .
O32 O 0.7792(4) 0.1029(8) 0.2587(3) 0.048(3) Uani 1 1 d . . .
O1W O 0.5000 0.0913(11) 0.7500 0.089(7) Uani 1 2 d S . .
O2W O 0.7012(5) 0.0740(7) 0.4661(4) 0.052(3) Uani 1 1 d . . .
O3W O 0.5499(6) 0.801(2) 0.1229(5) 0.168(11) Uani 1 1 d . . .
O4W O 0.8651(7) 0.7140(11) 0.7481(5) 0.102(5) Uani 1 1 d . . .
O5W O 0.5000 0.2918(16) 0.7500 0.211(19) Uani 1 2 d S . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
C1 N1 1.307(18) . ?
C1 C2 1.378(17) . ?
C1 H1 0.9300 . ?
C2 C3 1.381(17) . ?
C2 H2 0.9300 . ?
C3 C4 1.366(15) . ?
C3 C6 1.512(14) . ?
C4 C5 1.380(17) . ?
C4 H4 0.9300 . ?
C5 N1 1.338(18) . ?
C5 H5 0.9300 . ?
C6 O29 1.251(13) . ?
C6 O30 1.251(12) . ?
C7 N2 1.345(15) . ?
C7 C8 1.378(16) . ?
C7 H7 0.9300 . ?
C8 C9 1.375(17) . ?
C8 H8 0.9300 . ?
C9 C10 1.390(16) . ?
C9 C12 1.510(15) . ?
C10 C11 1.388(15) . ?
C10 H10 0.9300 . ?
C11 N2 1.310(14) . ?
C11 H11 0.9300 . ?
C12 O32 1.242(13) . ?
C12 O31 1.261(13) . ?
Cr1 O24 1.958(6) . ?
Cr1 O23 1.967(7) . ?
Cr1 O22 1.975(7) . ?
Cr1 O20 1.976(7) . ?
Cr1 O19 1.978(7) . ?
Cr1 O21 1.984(7) . ?
Gd1 O25 2.369(8) . ?
Gd1 O1 2.377(7) . ?
Gd1 O27 2.390(8) . ?
Gd1 O29 2.446(7) . ?
Gd1 O28 2.448(8) . ?
Gd1 O30 2.447(7) 2_656 ?
Gd1 O26 2.453(8) . ?
Gd1 O13 2.465(7) 4_646 ?
Gd1 O30 2.748(8) . ?
Mo1 O2 1.680(7) . ?
Mo1 O1 1.729(7) . ?
Mo1 O18 1.902(7) . ?
Mo1 O3 1.945(7) . ?
Mo1 O19 2.261(6) . ?
Mo1 O24 2.323(6) . ?
Mo2 O4 1.703(8) . ?
Mo2 O5 1.707(7) . ?
Mo2 O3 1.922(7) . ?
Mo2 O6 1.943(7) . ?
Mo2 O20 2.262(7) . ?
Mo2 O19 2.331(7) . ?
Mo3 O8 1.694(8) . ?
Mo3 O7 1.701(8) . ?
Mo3 O6 1.940(7) . ?
Mo3 O9 1.960(8) . ?
Mo3 O21 2.282(7) . ?
Mo3 O20 2.286(7) . ?
Mo4 O11 1.704(7) . ?
Mo4 O10 1.712(7) . ?
Mo4 O9 1.898(8) . ?
Mo4 O12 1.986(7) . ?
Mo4 O22 2.270(6) . ?
Mo4 O21 2.298(7) . ?
Mo5 O14 1.704(8) . ?
Mo5 O13 1.725(7) . ?
Mo5 O12 1.922(7) . ?
Mo5 O15 1.938(7) . ?
Mo5 O23 2.267(7) . ?
Mo5 O22 2.289(7) . ?
Mo6 O16 1.690(8) . ?
Mo6 O17 1.703(8) . ?
Mo6 O18 1.944(7) . ?
Mo6 O15 1.944(7) . ?
Mo6 O24 2.239(7) . ?
Mo6 O23 2.320(7) . ?
N1 H1B 0.8600 . ?
N2 H1A 0.8600 . ?
O13 Gd1 2.465(7) 4_656 ?
O30 Gd1 2.447(7) 2_656 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
N1 C1 C2 120.0(13) . . ?
N1 C1 H1 120.0 . . ?
C2 C1 H1 120.0 . . ?
C1 C2 C3 118.4(12) . . ?
C1 C2 H2 120.8 . . ?
C3 C2 H2 120.8 . . ?
C4 C3 C2 120.6(11) . . ?
C4 C3 C6 120.6(11) . . ?
C2 C3 C6 118.6(10) . . ?
C3 C4 C5 118.4(12) . . ?
C3 C4 H4 120.8 . . ?
C5 C4 H4 120.8 . . ?
N1 C5 C4 119.6(12) . . ?
N1 C5 H5 120.2 . . ?
C4 C5 H5 120.2 . . ?
O29 C6 O30 122.5(10) . . ?
O29 C6 C3 116.8(9) . . ?
O30 C6 C3 120.5(10) . . ?
N2 C7 C8 120.4(12) . . ?
N2 C7 H7 119.8 . . ?
C8 C7 H7 119.8 . . ?
C9 C8 C7 118.8(12) . . ?
C9 C8 H8 120.6 . . ?
C7 C8 H8 120.6 . . ?
C8 C9 C10 119.1(10) . . ?
C8 C9 C12 121.2(10) . . ?
C10 C9 C12 119.7(10) . . ?
C11 C10 C9 119.8(11) . . ?
C11 C10 H10 120.1 . . ?
C9 C10 H10 120.1 . . ?
N2 C11 C10 119.3(11) . . ?
N2 C11 H11 120.3 . . ?
C10 C11 H11 120.3 . . ?
O32 C12 O31 125.2(10) . . ?
O32 C12 C9 117.8(10) . . ?
O31 C12 C9 117.0(10) . . ?
O24 Cr1 O23 84.9(3) . . ?
O24 Cr1 O22 94.4(3) . . ?
O23 Cr1 O22 84.6(3) . . ?
O24 Cr1 O20 94.3(3) . . ?
O23 Cr1 O20 179.2(3) . . ?
O22 Cr1 O20 95.5(3) . . ?
O24 Cr1 O19 84.4(3) . . ?
O23 Cr1 O19 94.7(3) . . ?
O22 Cr1 O19 178.7(3) . . ?
O20 Cr1 O19 85.2(3) . . ?
O24 Cr1 O21 176.7(3) . . ?
O23 Cr1 O21 97.5(3) . . ?
O22 Cr1 O21 83.6(3) . . ?
O20 Cr1 O21 83.4(3) . . ?
O19 Cr1 O21 97.7(3) . . ?
O25 Gd1 O1 94.5(3) . . ?
O25 Gd1 O27 143.1(3) . . ?
O1 Gd1 O27 84.5(3) . . ?
O25 Gd1 O29 127.5(3) . . ?
O1 Gd1 O29 136.7(3) . . ?
O27 Gd1 O29 68.4(3) . . ?
O25 Gd1 O28 136.6(3) . . ?
O1 Gd1 O28 67.7(3) . . ?
O27 Gd1 O28 76.7(3) . . ?
O29 Gd1 O28 73.4(3) . . ?
O25 Gd1 O30 67.4(3) . 2_656 ?
O1 Gd1 O30 84.6(3) . 2_656 ?
O27 Gd1 O30 148.4(3) . 2_656 ?
O29 Gd1 O30 100.9(3) . 2_656 ?
O28 Gd1 O30 71.7(3) . 2_656 ?
O25 Gd1 O26 72.7(3) . . ?
O1 Gd1 O26 68.7(2) . . ?
O27 Gd1 O26 72.7(3) . . ?
O29 Gd1 O26 128.2(3) . . ?
O28 Gd1 O26 128.3(3) . . ?
O30 Gd1 O26 129.4(3) 2_656 . ?
O25 Gd1 O13 75.2(3) . 4_646 ?
O1 Gd1 O13 138.0(2) . 4_646 ?
O27 Gd1 O13 81.1(3) . 4_646 ?
O29 Gd1 O13 72.0(3) . 4_646 ?
O28 Gd1 O13 143.8(3) . 4_646 ?
O30 Gd1 O13 125.2(2) 2_656 4_646 ?
O26 Gd1 O13 69.3(2) . 4_646 ?
O25 Gd1 O30 81.6(3) . . ?
O1 Gd1 O30 148.8(2) . . ?
O27 Gd1 O30 116.8(2) . . ?
O29 Gd1 O30 49.5(2) . . ?
O28 Gd1 O30 94.0(2) . . ?
O30 Gd1 O30 65.3(3) 2_656 . ?
O26 Gd1 O30 137.0(2) . . ?
O13 Gd1 O30 71.1(2) 4_646 . ?
O2 Mo1 O1 104.9(4) . . ?
O2 Mo1 O18 102.2(3) . . ?
O1 Mo1 O18 102.1(3) . . ?
O2 Mo1 O3 98.6(3) . . ?
O1 Mo1 O3 94.7(3) . . ?
O18 Mo1 O3 148.8(3) . . ?
O2 Mo1 O19 91.0(3) . . ?
O1 Mo1 O19 161.4(3) . . ?
O18 Mo1 O19 83.5(3) . . ?
O3 Mo1 O19 73.0(3) . . ?
O2 Mo1 O24 160.5(3) . . ?
O1 Mo1 O24 94.5(3) . . ?
O18 Mo1 O24 70.8(3) . . ?
O3 Mo1 O24 81.9(3) . . ?
O19 Mo1 O24 70.4(2) . . ?
O4 Mo2 O5 105.9(4) . . ?
O4 Mo2 O3 101.4(3) . . ?
O5 Mo2 O3 100.3(3) . . ?
O4 Mo2 O6 96.6(3) . . ?
O5 Mo2 O6 100.0(3) . . ?
O3 Mo2 O6 147.9(3) . . ?
O4 Mo2 O20 158.1(3) . . ?
O5 Mo2 O20 94.9(3) . . ?
O3 Mo2 O20 81.3(3) . . ?
O6 Mo2 O20 72.5(3) . . ?
O4 Mo2 O19 88.8(3) . . ?
O5 Mo2 O19 164.7(3) . . ?
O3 Mo2 O19 71.8(3) . . ?
O6 Mo2 O19 82.4(3) . . ?
O20 Mo2 O19 71.3(2) . . ?
O8 Mo3 O7 104.2(4) . . ?
O8 Mo3 O6 98.7(4) . . ?
O7 Mo3 O6 102.5(4) . . ?
O8 Mo3 O9 100.5(4) . . ?
O7 Mo3 O9 97.4(4) . . ?
O6 Mo3 O9 147.9(3) . . ?
O8 Mo3 O21 97.2(3) . . ?
O7 Mo3 O21 157.5(3) . . ?
O6 Mo3 O21 81.1(3) . . ?
O9 Mo3 O21 71.2(3) . . ?
O8 Mo3 O20 165.1(3) . . ?
O7 Mo3 O20 89.4(3) . . ?
O6 Mo3 O20 72.0(3) . . ?
O9 Mo3 O20 83.5(3) . . ?
O21 Mo3 O20 70.4(2) . . ?
O11 Mo4 O10 105.9(4) . . ?
O11 Mo4 O9 99.8(4) . . ?
O10 Mo4 O9 102.7(4) . . ?
O11 Mo4 O12 100.3(4) . . ?
O10 Mo4 O12 93.9(3) . . ?
O9 Mo4 O12 149.2(3) . . ?
O11 Mo4 O22 92.0(3) . . ?
O10 Mo4 O22 158.5(3) . . ?
O9 Mo4 O22 85.3(3) . . ?
O12 Mo4 O22 70.8(2) . . ?
O11 Mo4 O21 160.9(3) . . ?
O10 Mo4 O21 92.8(3) . . ?
O9 Mo4 O21 71.9(3) . . ?
O12 Mo4 O21 81.7(3) . . ?
O22 Mo4 O21 70.6(2) . . ?
O14 Mo5 O13 106.0(4) . . ?
O14 Mo5 O12 97.4(3) . . ?
O13 Mo5 O12 102.0(3) . . ?
O14 Mo5 O15 102.0(3) . . ?
O13 Mo5 O15 94.5(3) . . ?
O12 Mo5 O15 149.9(3) . . ?
O14 Mo5 O23 90.9(3) . . ?
O13 Mo5 O23 160.6(3) . . ?
O12 Mo5 O23 84.8(3) . . ?
O15 Mo5 O23 72.2(3) . . ?
O14 Mo5 O22 159.3(3) . . ?
O13 Mo5 O22 93.6(3) . . ?
O12 Mo5 O22 71.5(3) . . ?
O15 Mo5 O22 82.7(3) . . ?
O23 Mo5 O22 71.2(2) . . ?
O16 Mo6 O17 105.4(4) . . ?
O16 Mo6 O18 96.1(3) . . ?
O17 Mo6 O18 100.8(3) . . ?
O16 Mo6 O15 100.0(3) . . ?
O17 Mo6 O15 98.3(3) . . ?
O18 Mo6 O15 150.7(3) . . ?
O16 Mo6 O24 159.1(3) . . ?
O17 Mo6 O24 93.9(3) . . ?
O18 Mo6 O24 72.1(3) . . ?
O15 Mo6 O24 84.7(3) . . ?
O16 Mo6 O23 91.1(3) . . ?
O17 Mo6 O23 161.8(3) . . ?
O18 Mo6 O23 84.5(3) . . ?
O15 Mo6 O23 70.9(3) . . ?
O24 Mo6 O23 71.0(2) . . ?
C1 N1 C5 122.9(11) . . ?
C1 N1 H1B 118.5 . . ?
C5 N1 H1B 118.5 . . ?
C11 N2 C7 122.5(10) . . ?
C11 N2 H1A 118.7 . . ?
C7 N2 H1A 118.7 . . ?
Mo1 O1 Gd1 163.9(4) . . ?
Mo2 O3 Mo1 117.5(3) . . ?
Mo3 O6 Mo2 115.7(4) . . ?
Mo4 O9 Mo3 119.5(4) . . ?
Mo5 O12 Mo4 118.0(3) . . ?
Mo5 O13 Gd1 158.5(4) . 4_656 ?
Mo5 O15 Mo6 119.4(3) . . ?
Mo1 O18 Mo6 119.6(3) . . ?
Cr1 O19 Mo1 103.4(3) . . ?
Cr1 O19 Mo2 100.5(3) . . ?
Mo1 O19 Mo2 92.1(2) . . ?
Cr1 O20 Mo2 103.0(3) . . ?
Cr1 O20 Mo3 103.2(3) . . ?
Mo2 O20 Mo3 92.6(2) . . ?
Cr1 O21 Mo3 103.0(3) . . ?
Cr1 O21 Mo4 102.3(3) . . ?
Mo3 O21 Mo4 93.4(3) . . ?
Cr1 O22 Mo4 103.6(3) . . ?
Cr1 O22 Mo5 101.6(3) . . ?
Mo4 O22 Mo5 94.6(2) . . ?
Cr1 O23 Mo5 102.6(3) . . ?
Cr1 O23 Mo6 100.5(3) . . ?
Mo5 O23 Mo6 93.9(2) . . ?
Cr1 O24 Mo6 103.7(3) . . ?
Cr1 O24 Mo1 101.8(3) . . ?
Mo6 O24 Mo1 93.5(2) . . ?
C6 O29 Gd1 98.6(6) . . ?
C6 O30 Gd1 135.4(7) . 2_656 ?
C6 O30 Gd1 84.6(6) . . ?
Gd1 O30 Gd1 114.5(3) 2_656 . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
N1 C1 C2 C3 2.7(18) . . . . ?
C1 C2 C3 C4 -1.8(17) . . . . ?
C1 C2 C3 C6 173.2(10) . . . . ?
C2 C3 C4 C5 0.9(18) . . . . ?
C6 C3 C4 C5 -174.0(11) . . . . ?
C3 C4 C5 N1 -1(2) . . . . ?
C4 C3 C6 O29 26.0(15) . . . . ?
C2 C3 C6 O29 -149.0(10) . . . . ?
C4 C3 C6 O30 -158.9(11) . . . . ?
C2 C3 C6 O30 26.0(15) . . . . ?
N2 C7 C8 C9 -1(2) . . . . ?
C7 C8 C9 C10 2(2) . . . . ?
C7 C8 C9 C12 -178.0(12) . . . . ?
C8 C9 C10 C11 -2.6(18) . . . . ?
C12 C9 C10 C11 177.3(11) . . . . ?
C9 C10 C11 N2 2.7(18) . . . . ?
C8 C9 C12 O32 158.0(13) . . . . ?
C10 C9 C12 O32 -21.9(17) . . . . ?
C8 C9 C12 O31 -20.5(17) . . . . ?
C10 C9 C12 O31 159.7(11) . . . . ?
C2 C1 N1 C5 -3(2) . . . . ?
C4 C5 N1 C1 2(2) . . . . ?
C10 C11 N2 C7 -2.3(17) . . . . ?
C8 C7 N2 C11 1.6(19) . . . . ?
O2 Mo1 O1 Gd1 98.9(16) . . . . ?
O18 Mo1 O1 Gd1 -154.8(15) . . . . ?
O3 Mo1 O1 Gd1 -1.2(16) . . . . ?
O19 Mo1 O1 Gd1 -49(2) . . . . ?
O24 Mo1 O1 Gd1 -83.5(16) . . . . ?
O25 Gd1 O1 Mo1 -62.1(16) . . . . ?
O27 Gd1 O1 Mo1 80.9(16) . . . . ?
O29 Gd1 O1 Mo1 131.0(15) . . . . ?
O28 Gd1 O1 Mo1 158.8(17) . . . . ?
O30 Gd1 O1 Mo1 -128.8(16) 2_656 . . . ?
O26 Gd1 O1 Mo1 7.4(15) . . . . ?
O13 Gd1 O1 Mo1 10.7(18) 4_646 . . . ?
O30 Gd1 O1 Mo1 -143.2(14) . . . . ?
O4 Mo2 O3 Mo1 -64.0(5) . . . . ?
O5 Mo2 O3 Mo1 -172.6(4) . . . . ?
O6 Mo2 O3 Mo1 58.8(7) . . . . ?
O20 Mo2 O3 Mo1 93.9(4) . . . . ?
O19 Mo2 O3 Mo1 20.9(3) . . . . ?
O2 Mo1 O3 Mo2 67.0(5) . . . . ?
O1 Mo1 O3 Mo2 172.8(4) . . . . ?
O18 Mo1 O3 Mo2 -64.4(7) . . . . ?
O19 Mo1 O3 Mo2 -21.4(3) . . . . ?
O24 Mo1 O3 Mo2 -93.3(4) . . . . ?
O8 Mo3 O6 Mo2 168.4(4) . . . . ?
O7 Mo3 O6 Mo2 61.7(5) . . . . ?
O9 Mo3 O6 Mo2 -65.4(7) . . . . ?
O21 Mo3 O6 Mo2 -95.6(4) . . . . ?
O20 Mo3 O6 Mo2 -23.5(3) . . . . ?
O4 Mo2 O6 Mo3 -175.8(4) . . . . ?
O5 Mo2 O6 Mo3 -68.3(5) . . . . ?
O3 Mo2 O6 Mo3 60.2(7) . . . . ?
O20 Mo2 O6 Mo3 23.7(3) . . . . ?
O19 Mo2 O6 Mo3 96.4(4) . . . . ?
O11 Mo4 O9 Mo3 -179.7(4) . . . . ?
O10 Mo4 O9 Mo3 -70.8(5) . . . . ?
O12 Mo4 O9 Mo3 50.3(8) . . . . ?
O22 Mo4 O9 Mo3 89.1(4) . . . . ?
O21 Mo4 O9 Mo3 18.0(4) . . . . ?
O8 Mo3 O9 Mo4 75.8(5) . . . . ?
O7 Mo3 O9 Mo4 -178.2(5) . . . . ?
O6 Mo3 O9 Mo4 -50.0(8) . . . . ?
O21 Mo3 O9 Mo4 -18.2(4) . . . . ?
O20 Mo3 O9 Mo4 -89.7(4) . . . . ?
O14 Mo5 O12 Mo4 178.1(4) . . . . ?
O13 Mo5 O12 Mo4 70.0(4) . . . . ?
O15 Mo5 O12 Mo4 -51.8(7) . . . . ?
O23 Mo5 O12 Mo4 -91.7(4) . . . . ?
O22 Mo5 O12 Mo4 -19.8(3) . . . . ?
O11 Mo4 O12 Mo5 -68.5(4) . . . . ?
O10 Mo4 O12 Mo5 -175.5(4) . . . . ?
O9 Mo4 O12 Mo5 61.4(7) . . . . ?
O22 Mo4 O12 Mo5 20.0(3) . . . . ?
O21 Mo4 O12 Mo5 92.3(4) . . . . ?
O14 Mo5 O13 Gd1 88.6(11) . . . 4_656 ?
O12 Mo5 O13 Gd1 -170.0(11) . . . 4_656 ?
O15 Mo5 O13 Gd1 -15.3(11) . . . 4_656 ?
O23 Mo5 O13 Gd1 -60.9(17) . . . 4_656 ?
O22 Mo5 O13 Gd1 -98.2(11) . . . 4_656 ?
O14 Mo5 O15 Mo6 69.9(5) . . . . ?
O13 Mo5 O15 Mo6 177.3(4) . . . . ?
O12 Mo5 O15 Mo6 -59.2(7) . . . . ?
O23 Mo5 O15 Mo6 -17.1(3) . . . . ?
O22 Mo5 O15 Mo6 -89.6(4) . . . . ?
O16 Mo6 O15 Mo5 -70.9(5) . . . . ?
O17 Mo6 O15 Mo5 -178.3(4) . . . . ?
O18 Mo6 O15 Mo5 51.4(8) . . . . ?
O24 Mo6 O15 Mo5 88.5(4) . . . . ?
O23 Mo6 O15 Mo5 16.8(3) . . . . ?
O2 Mo1 O18 Mo6 -178.9(4) . . . . ?
O1 Mo1 O18 Mo6 72.7(4) . . . . ?
O3 Mo1 O18 Mo6 -48.3(7) . . . . ?
O19 Mo1 O18 Mo6 -89.3(4) . . . . ?
O24 Mo1 O18 Mo6 -17.8(3) . . . . ?
O16 Mo6 O18 Mo1 -179.3(4) . . . . ?
O17 Mo6 O18 Mo1 -72.3(5) . . . . ?
O15 Mo6 O18 Mo1 57.6(7) . . . . ?
O24 Mo6 O18 Mo1 18.4(3) . . . . ?
O23 Mo6 O18 Mo1 90.2(4) . . . . ?
O24 Cr1 O19 Mo1 -1.7(3) . . . . ?
O23 Cr1 O19 Mo1 -86.0(3) . . . . ?
O20 Cr1 O19 Mo1 93.1(3) . . . . ?
O21 Cr1 O19 Mo1 175.8(3) . . . . ?
O24 Cr1 O19 Mo2 -96.4(3) . . . . ?
O23 Cr1 O19 Mo2 179.3(3) . . . . ?
O20 Cr1 O19 Mo2 -1.6(3) . . . . ?
O21 Cr1 O19 Mo2 81.1(3) . . . . ?
O2 Mo1 O19 Cr1 175.5(4) . . . . ?
O1 Mo1 O19 Cr1 -35.6(11) . . . . ?
O18 Mo1 O19 Cr1 73.4(3) . . . . ?
O3 Mo1 O19 Cr1 -85.8(3) . . . . ?
O24 Mo1 O19 Cr1 1.5(3) . . . . ?
O2 Mo1 O19 Mo2 -83.2(3) . . . . ?
O1 Mo1 O19 Mo2 65.7(10) . . . . ?
O18 Mo1 O19 Mo2 174.7(3) . . . . ?
O3 Mo1 O19 Mo2 15.5(3) . . . . ?
O24 Mo1 O19 Mo2 102.8(3) . . . . ?
O4 Mo2 O19 Cr1 -169.3(3) . . . . ?
O5 Mo2 O19 Cr1 27.6(13) . . . . ?
O3 Mo2 O19 Cr1 88.2(3) . . . . ?
O6 Mo2 O19 Cr1 -72.6(3) . . . . ?
O20 Mo2 O19 Cr1 1.4(2) . . . . ?
O4 Mo2 O19 Mo1 86.7(3) . . . . ?
O5 Mo2 O19 Mo1 -76.4(12) . . . . ?
O3 Mo2 O19 Mo1 -15.8(3) . . . . ?
O6 Mo2 O19 Mo1 -176.6(3) . . . . ?
O20 Mo2 O19 Mo1 -102.6(3) . . . . ?
O24 Cr1 O20 Mo2 85.6(3) . . . . ?
O22 Cr1 O20 Mo2 -179.5(3) . . . . ?
O19 Cr1 O20 Mo2 1.6(3) . . . . ?
O21 Cr1 O20 Mo2 -96.7(3) . . . . ?
O24 Cr1 O20 Mo3 -178.6(3) . . . . ?
O22 Cr1 O20 Mo3 -83.7(3) . . . . ?
O19 Cr1 O20 Mo3 97.5(3) . . . . ?
O21 Cr1 O20 Mo3 -0.8(3) . . . . ?
O4 Mo2 O20 Cr1 23.9(10) . . . . ?
O5 Mo2 O20 Cr1 -174.8(4) . . . . ?
O3 Mo2 O20 Cr1 -75.1(3) . . . . ?
O6 Mo2 O20 Cr1 86.3(3) . . . . ?
O19 Mo2 O20 Cr1 -1.5(3) . . . . ?
O4 Mo2 O20 Mo3 -80.3(9) . . . . ?
O5 Mo2 O20 Mo3 81.1(3) . . . . ?
O3 Mo2 O20 Mo3 -179.2(3) . . . . ?
O6 Mo2 O20 Mo3 -17.9(3) . . . . ?
O19 Mo2 O20 Mo3 -105.6(3) . . . . ?
O8 Mo3 O20 Cr1 -33.5(15) . . . . ?
O7 Mo3 O20 Cr1 170.6(4) . . . . ?
O6 Mo3 O20 Cr1 -86.0(3) . . . . ?
O9 Mo3 O20 Cr1 73.1(3) . . . . ?
O21 Mo3 O20 Cr1 0.8(3) . . . . ?
O8 Mo3 O20 Mo2 70.5(15) . . . . ?
O7 Mo3 O20 Mo2 -85.4(3) . . . . ?
O6 Mo3 O20 Mo2 18.0(3) . . . . ?
O9 Mo3 O20 Mo2 177.1(3) . . . . ?
O21 Mo3 O20 Mo2 104.8(3) . . . . ?
O23 Cr1 O21 Mo3 -179.2(3) . . . . ?
O22 Cr1 O21 Mo3 97.2(3) . . . . ?
O20 Cr1 O21 Mo3 0.8(3) . . . . ?
O19 Cr1 O21 Mo3 -83.4(3) . . . . ?
O23 Cr1 O21 Mo4 84.3(3) . . . . ?
O22 Cr1 O21 Mo4 0.7(3) . . . . ?
O20 Cr1 O21 Mo4 -95.6(3) . . . . ?
O19 Cr1 O21 Mo4 -179.8(3) . . . . ?
O8 Mo3 O21 Cr1 170.9(4) . . . . ?
O7 Mo3 O21 Cr1 -28.0(10) . . . . ?
O6 Mo3 O21 Cr1 73.1(3) . . . . ?
O9 Mo3 O21 Cr1 -90.4(3) . . . . ?
O20 Mo3 O21 Cr1 -0.8(3) . . . . ?
O8 Mo3 O21 Mo4 -85.7(4) . . . . ?
O7 Mo3 O21 Mo4 75.4(9) . . . . ?
O6 Mo3 O21 Mo4 176.6(3) . . . . ?
O9 Mo3 O21 Mo4 13.0(3) . . . . ?
O20 Mo3 O21 Mo4 102.7(3) . . . . ?
O11 Mo4 O21 Cr1 24.3(12) . . . . ?
O10 Mo4 O21 Cr1 -166.8(4) . . . . ?
O9 Mo4 O21 Cr1 90.7(3) . . . . ?
O12 Mo4 O21 Cr1 -73.2(3) . . . . ?
O22 Mo4 O21 Cr1 -0.7(3) . . . . ?
O11 Mo4 O21 Mo3 -79.8(11) . . . . ?
O10 Mo4 O21 Mo3 89.1(3) . . . . ?
O9 Mo4 O21 Mo3 -13.4(3) . . . . ?
O12 Mo4 O21 Mo3 -177.3(3) . . . . ?
O22 Mo4 O21 Mo3 -104.8(3) . . . . ?
O24 Cr1 O22 Mo4 176.7(3) . . . . ?
O23 Cr1 O22 Mo4 -98.9(3) . . . . ?
O20 Cr1 O22 Mo4 81.9(3) . . . . ?
O21 Cr1 O22 Mo4 -0.7(3) . . . . ?
O24 Cr1 O22 Mo5 -85.6(3) . . . . ?
O23 Cr1 O22 Mo5 -1.2(3) . . . . ?
O20 Cr1 O22 Mo5 179.6(3) . . . . ?
O21 Cr1 O22 Mo5 97.0(3) . . . . ?
O11 Mo4 O22 Cr1 -171.4(4) . . . . ?
O10 Mo4 O22 Cr1 41.6(10) . . . . ?
O9 Mo4 O22 Cr1 -71.8(3) . . . . ?
O12 Mo4 O22 Cr1 88.4(3) . . . . ?
O21 Mo4 O22 Cr1 0.7(3) . . . . ?
O11 Mo4 O22 Mo5 85.5(3) . . . . ?
O10 Mo4 O22 Mo5 -61.5(9) . . . . ?
O9 Mo4 O22 Mo5 -174.9(3) . . . . ?
O12 Mo4 O22 Mo5 -14.8(2) . . . . ?
O21 Mo4 O22 Mo5 -102.5(3) . . . . ?
O14 Mo5 O22 Cr1 -30.0(10) . . . . ?
O13 Mo5 O22 Cr1 168.8(3) . . . . ?
O12 Mo5 O22 Cr1 -89.7(3) . . . . ?
O15 Mo5 O22 Cr1 74.8(3) . . . . ?
O23 Mo5 O22 Cr1 1.1(2) . . . . ?
O14 Mo5 O22 Mo4 74.9(9) . . . . ?
O13 Mo5 O22 Mo4 -86.3(3) . . . . ?
O12 Mo5 O22 Mo4 15.2(2) . . . . ?
O15 Mo5 O22 Mo4 179.7(3) . . . . ?
O23 Mo5 O22 Mo4 106.0(3) . . . . ?
O24 Cr1 O23 Mo5 96.2(3) . . . . ?
O22 Cr1 O23 Mo5 1.2(3) . . . . ?
O19 Cr1 O23 Mo5 -179.9(3) . . . . ?
O21 Cr1 O23 Mo5 -81.5(3) . . . . ?
O24 Cr1 O23 Mo6 -0.3(3) . . . . ?
O22 Cr1 O23 Mo6 -95.2(3) . . . . ?
O19 Cr1 O23 Mo6 83.6(3) . . . . ?
O21 Cr1 O23 Mo6 -178.0(3) . . . . ?
O14 Mo5 O23 Cr1 168.4(4) . . . . ?
O13 Mo5 O23 Cr1 -40.9(10) . . . . ?
O12 Mo5 O23 Cr1 71.0(3) . . . . ?
O15 Mo5 O23 Cr1 -89.3(3) . . . . ?
O22 Mo5 O23 Cr1 -1.1(2) . . . . ?
O14 Mo5 O23 Mo6 -90.0(3) . . . . ?
O13 Mo5 O23 Mo6 60.8(10) . . . . ?
O12 Mo5 O23 Mo6 172.7(3) . . . . ?
O15 Mo5 O23 Mo6 12.4(2) . . . . ?
O22 Mo5 O23 Mo6 100.6(3) . . . . ?
O16 Mo6 O23 Cr1 -168.7(4) . . . . ?
O17 Mo6 O23 Cr1 35.6(11) . . . . ?
O18 Mo6 O23 Cr1 -72.7(3) . . . . ?
O15 Mo6 O23 Cr1 91.1(3) . . . . ?
O24 Mo6 O23 Cr1 0.2(2) . . . . ?
O16 Mo6 O23 Mo5 87.7(3) . . . . ?
O17 Mo6 O23 Mo5 -68.0(11) . . . . ?
O18 Mo6 O23 Mo5 -176.3(3) . . . . ?
O15 Mo6 O23 Mo5 -12.5(2) . . . . ?
O24 Mo6 O23 Mo5 -103.4(3) . . . . ?
O23 Cr1 O24 Mo6 0.3(3) . . . . ?
O22 Cr1 O24 Mo6 84.4(3) . . . . ?
O20 Cr1 O24 Mo6 -179.7(3) . . . . ?
O19 Cr1 O24 Mo6 -95.0(3) . . . . ?
O23 Cr1 O24 Mo1 96.9(3) . . . . ?
O22 Cr1 O24 Mo1 -179.0(3) . . . . ?
O20 Cr1 O24 Mo1 -83.1(3) . . . . ?
O19 Cr1 O24 Mo1 1.6(3) . . . . ?
O16 Mo6 O24 Cr1 32.2(10) . . . . ?
O17 Mo6 O24 Cr1 -169.8(4) . . . . ?
O18 Mo6 O24 Cr1 90.0(3) . . . . ?
O15 Mo6 O24 Cr1 -71.9(3) . . . . ?
O23 Mo6 O24 Cr1 -0.2(2) . . . . ?
O16 Mo6 O24 Mo1 -70.8(9) . . . . ?
O17 Mo6 O24 Mo1 87.1(3) . . . . ?
O18 Mo6 O24 Mo1 -13.0(2) . . . . ?
O15 Mo6 O24 Mo1 -174.9(3) . . . . ?
O23 Mo6 O24 Mo1 -103.3(3) . . . . ?
O2 Mo1 O24 Cr1 -19.7(11) . . . . ?
O1 Mo1 O24 Cr1 167.4(3) . . . . ?
O18 Mo1 O24 Cr1 -91.3(3) . . . . ?
O3 Mo1 O24 Cr1 73.3(3) . . . . ?
O19 Mo1 O24 Cr1 -1.5(3) . . . . ?
O2 Mo1 O24 Mo6 85.1(10) . . . . ?
O1 Mo1 O24 Mo6 -87.9(3) . . . . ?
O18 Mo1 O24 Mo6 13.4(2) . . . . ?
O3 Mo1 O24 Mo6 178.0(3) . . . . ?
O19 Mo1 O24 Mo6 103.3(3) . . . . ?
O30 C6 O29 Gd1 -24.3(11) . . . . ?
C3 C6 O29 Gd1 150.7(7) . . . . ?
O25 Gd1 O29 C6 -14.2(8) . . . . ?
O1 Gd1 O29 C6 149.2(6) . . . . ?
O27 Gd1 O29 C6 -155.6(7) . . . . ?
O28 Gd1 O29 C6 122.5(7) . . . . ?
O30 Gd1 O29 C6 55.5(7) 2_656 . . . ?
O26 Gd1 O29 C6 -111.5(7) . . . . ?
O13 Gd1 O29 C6 -68.2(6) 4_646 . . . ?
O30 Gd1 O29 C6 12.0(6) . . . . ?
O29 C6 O30 Gd1 -98.5(12) . . . 2_656 ?
C3 C6 O30 Gd1 86.7(12) . . . 2_656 ?
O29 C6 O30 Gd1 21.3(10) . . . . ?
C3 C6 O30 Gd1 -153.5(9) . . . . ?
O25 Gd1 O30 C6 147.4(6) . . . . ?
O1 Gd1 O30 C6 -127.9(6) . . . . ?
O27 Gd1 O30 C6 1.1(7) . . . . ?
O29 Gd1 O30 C6 -11.9(6) . . . . ?
O28 Gd1 O30 C6 -76.0(6) . . . . ?
O30 Gd1 O30 C6 -143.8(5) 2_656 . . . ?
O26 Gd1 O30 C6 94.1(6) . . . . ?
O13 Gd1 O30 C6 70.2(6) 4_646 . . . ?
O25 Gd1 O30 Gd1 -74.6(3) . . . 2_656 ?
O1 Gd1 O30 Gd1 10.1(6) . . . 2_656 ?
O27 Gd1 O30 Gd1 139.1(3) . . . 2_656 ?
O29 Gd1 O30 Gd1 126.1(4) . . . 2_656 ?
O28 Gd1 O30 Gd1 62.0(3) . . . 2_656 ?
O30 Gd1 O30 Gd1 -5.8(4) 2_656 . . 2_656 ?
O26 Gd1 O30 Gd1 -127.9(3) . . . 2_656 ?
O13 Gd1 O30 Gd1 -151.8(4) 4_646 . . 2_656 ?

_diffrn_measured_fraction_theta_max 0.999
_diffrn_reflns_theta_full        25.00
_diffrn_measured_fraction_theta_full 0.999
_refine_diff_density_max         1.493
_refine_diff_density_min         -1.221
_refine_diff_density_rms         0.213
_database_code_depnum_ccdc_archive 'CCDC 806605'
#######################################################################
#
#                 Cambridge Crystallographic Data Centre
#                                CCDC 
# 
#######################################################################
# 
#  This CIF contains data from an original supplementary publication
#  deposited with the CCDC, and may include chemical, crystal,
#  experimental, refinement, atomic coordinates,
#  anisotropic displacement parameters and molecular geometry data,
#  as required by the journal to which it was submitted.
#
#  This CIF is provided on the understanding that it is used for bona
#  fide research purposes only. It may contain copyright material
#  of the CCDC or of third parties, and may not be copied or further
#  disseminated in any form, whether machine-readable or not,
#  except for the purpose of generating routine backup copies
#  on your local computer system.
# 
#  For further information on the CCDC, data deposition and
#  data retrieval see:
#                         www.ccdc.cam.ac.uk
#
#  Bona fide researchers may freely download Mercury and enCIFer
#  from this site to visualise CIF-encoded structures and 
#  to carry out CIF format checking respectively.
#
data_4

_audit_creation_method           'SHELXTL-NT2000 ver.6.12'
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'Cr Mo6 O30 Tb, 2(C6 H5 N O2), 4(O)'
_chemical_formula_sum            'C12 H10 Cr Mo6 N2 O38 Tb'
_chemical_formula_weight         1576.79

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Tb Tb -0.1723 4.1537 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cr Cr 0.3209 0.6236 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Monoclinic
_symmetry_space_group_name_H-M   C2/c
_symmetry_space_group_name_Hall  '-C 2yc'

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'

_cell_length_a                   18.389(2)
_cell_length_b                   12.5427(14)
_cell_length_c                   17.963(2)
_cell_angle_alpha                90.00
_cell_angle_beta                 104.117(2)
_cell_angle_gamma                90.00
_cell_volume                     4018.0(8)
_cell_formula_units_Z            4
_cell_measurement_temperature    298(2)
_cell_measurement_reflns_used    7862
_cell_measurement_theta_min      2.44
_cell_measurement_theta_max      28.30

_exptl_crystal_description       block
_exptl_crystal_colour            pink
_exptl_crystal_size_max          0.56
_exptl_crystal_size_mid          0.45
_exptl_crystal_size_min          0.37
_exptl_crystal_density_meas      2.508
_exptl_crystal_density_diffrn    2.607
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             2964
_exptl_absorpt_coefficient_mu    3.922
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.138
_exptl_absorpt_correction_T_max  0.234
_exptl_absorpt_process_details   '(SADABS; Bruker, 2000)'

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      298(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            10273
_diffrn_reflns_av_R_equivalents  0.0211
_diffrn_reflns_av_sigmaI/netI    0.0237
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_h_max       21
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_theta_min         1.99
_diffrn_reflns_theta_max         25.00
_reflns_number_total             3533
_reflns_number_gt                3456
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0444P)²+27.0766P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         3533
_refine_ls_number_parameters     273
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0329
_refine_ls_R_factor_gt           0.0313
_refine_ls_wR_factor_ref         0.0972
_refine_ls_wR_factor_gt          0.0878
_refine_ls_goodness_of_fit_ref   1.297
_refine_ls_restrained_S_all      1.297
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
C1 C 0.1597(4) 0.0501(5) 0.5284(4) 0.0373(16) Uani 1 1 d . . .
C2 C 0.1539(4) 0.1665(5) 0.5466(4) 0.0332(15) Uani 1 1 d . . .
C3 C 0.1468(5) 0.2037(6) 0.6177(4) 0.0449(19) Uani 1 1 d . . .
H3 H 0.1451 0.1561 0.6569 0.054 Uiso 1 1 calc R . .
C4 C 0.1424(5) 0.3110(6) 0.6290(4) 0.0451(19) Uani 1 1 d . . .
H4 H 0.1372 0.3367 0.6760 0.054 Uiso 1 1 calc R . .
C5 C 0.1522(4) 0.3468(6) 0.5042(4) 0.0387(17) Uani 1 1 d . . .
H5 H 0.1537 0.3971 0.4665 0.046 Uiso 1 1 calc R . .
C6 C 0.1570(4) 0.2400(6) 0.4891(4) 0.0380(16) Uani 1 1 d . . .
H6 H 0.1622 0.2171 0.4414 0.046 Uiso 1 1 calc R . .
Cr1 Cr 0.2500 0.7500 0.5000 0.0181(3) Uani 1 2 d S . .
Mo2 Mo 0.29085(3) 0.83957(4) 0.34030(3) 0.02149(15) Uani 1 1 d . . .
Mo3 Mo 0.38132(3) 0.73633(4) 0.66264(3) 0.02183(15) Uani 1 1 d . . .
Mo4 Mo 0.42446(3) 0.82572(4) 0.50504(3) 0.02403(15) Uani 1 1 d . . .
N1 N 0.1454(3) 0.3779(4) 0.5735(3) 0.0352(13) Uani 1 1 d . . .
H1 H 0.1430 0.4451 0.5822 0.042 Uiso 1 1 calc R . .
O1 O 0.3511(3) 0.7841(4) 0.2929(3) 0.0350(11) Uani 1 1 d . . .
O2 O 0.2564(3) 0.9523(3) 0.2899(3) 0.0320(10) Uani 1 1 d . . .
O3 O 0.3605(2) 0.9112(3) 0.4236(2) 0.0244(9) Uani 1 1 d . . .
O4 O 0.4845(3) 0.7717(4) 0.4560(3) 0.0392(12) Uani 1 1 d . . .
O5 O 0.4713(3) 0.9293(4) 0.5574(3) 0.0390(11) Uani 1 1 d . . .
O6 O 0.4343(2) 0.7168(3) 0.5834(2) 0.0265(9) Uani 1 1 d . . .
O7 O 0.4267(3) 0.8417(4) 0.7109(3) 0.0360(11) Uani 1 1 d . . .
O8 O 0.4180(2) 0.6234(3) 0.7143(3) 0.0290(9) Uani 1 1 d . . .
O9 O 0.2106(2) 0.7419(3) 0.3054(2) 0.0252(9) Uani 1 1 d . . .
O10 O 0.2114(2) 0.8548(3) 0.4178(2) 0.0206(8) Uani 1 1 d . . .
O11 O 0.3268(2) 0.7223(3) 0.4416(2) 0.0218(8) Uani 1 1 d . . .
O12 O 0.3266(2) 0.8441(3) 0.5644(2) 0.0212(8) Uani 1 1 d . . .
O13 O 0.5178(3) 0.3201(4) 0.8304(3) 0.0472(13) Uani 1 1 d . . .
O14 O 0.4894(3) 0.5278(4) 0.8746(3) 0.0362(11) Uani 1 1 d . . .
O15 O 0.6247(3) 0.4193(4) 0.7542(3) 0.0411(12) Uani 1 1 d . . .
O16 O 0.1348(3) -0.0165(4) 0.5696(3) 0.0453(13) Uani 1 1 d . . .
O17 O 0.1892(4) 0.0304(4) 0.4740(4) 0.0569(16) Uani 1 1 d . . .
O1W O 0.3088(4) 0.0258(5) 0.6440(4) 0.0649(18) Uani 1 1 d . . .
O2W O 0.4602(9) 0.0954(12) 0.6754(6) 0.191(8) Uani 1 1 d . . .
Tb1 Tb 0.5000 0.47591(3) 0.7500 0.02264(13) Uani 1 2 d S . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
C1 O17 1.254(9) . ?
C1 O16 1.272(9) . ?
C1 C2 1.506(9) . ?
C2 C3 1.395(10) . ?
C2 C6 1.397(10) . ?
C3 C4 1.366(10) . ?
C3 H3 0.9300 . ?
C4 N1 1.315(9) . ?
C4 H4 0.9300 . ?
C5 N1 1.340(9) . ?
C5 C6 1.373(10) . ?
C5 H5 0.9300 . ?
C6 H6 0.9300 . ?
Cr1 O10 1.975(4) 7_566 ?
Cr1 O10 1.975(4) . ?
Cr1 O12 1.980(4) . ?
Cr1 O12 1.980(4) 7_566 ?
Cr1 O11 1.985(4) . ?
Cr1 O11 1.986(4) 7_566 ?
Mo2 O1 1.702(4) . ?
Mo2 O2 1.715(4) . ?
Mo2 O9 1.904(4) . ?
Mo2 O3 1.937(4) . ?
Mo2 O10 2.259(4) . ?
Mo2 O11 2.307(4) . ?
Mo3 O7 1.686(5) . ?
Mo3 O8 1.737(4) . ?
Mo3 O6 1.926(4) . ?
Mo3 O9 1.932(4) 7_566 ?
Mo3 O12 2.257(4) . ?
Mo3 O10 2.258(4) 7_566 ?
Mo4 O5 1.708(5) . ?
Mo4 O4 1.712(5) . ?
Mo4 O6 1.939(4) . ?
Mo4 O3 1.958(4) . ?
Mo4 O11 2.282(4) . ?
Mo4 O12 2.316(4) . ?
N1 H1 0.8600 . ?
O8 Tb1 2.374(4) . ?
O9 Mo3 1.932(4) 7_566 ?
O10 Mo3 2.258(4) 7_566 ?
O13 Tb1 2.405(5) . ?
O14 Tb1 2.384(5) . ?
O15 Tb1 2.384(5) . ?
Tb1 O8 2.374(4) 2_656 ?
Tb1 O14 2.384(5) 2_656 ?
Tb1 O15 2.384(5) 2_656 ?
Tb1 O13 2.405(5) 2_656 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O17 C1 O16 127.6(7) . . ?
O17 C1 C2 115.3(6) . . ?
O16 C1 C2 117.1(6) . . ?
C3 C2 C6 119.1(6) . . ?
C3 C2 C1 123.4(6) . . ?
C6 C2 C1 117.5(6) . . ?
C4 C3 C2 119.3(7) . . ?
C4 C3 H3 120.4 . . ?
C2 C3 H3 120.4 . . ?
N1 C4 C3 120.0(7) . . ?
N1 C4 H4 120.0 . . ?
C3 C4 H4 120.0 . . ?
N1 C5 C6 119.5(7) . . ?
N1 C5 H5 120.2 . . ?
C6 C5 H5 120.2 . . ?
C5 C6 C2 118.8(7) . . ?
C5 C6 H6 120.6 . . ?
C2 C6 H6 120.6 . . ?
O10 Cr1 O10 179.999(2) 7_566 . ?
O10 Cr1 O12 83.43(16) 7_566 . ?
O10 Cr1 O12 96.57(16) . . ?
O10 Cr1 O12 96.57(16) 7_566 7_566 ?
O10 Cr1 O12 83.43(16) . 7_566 ?
O12 Cr1 O12 180.0 . 7_566 ?
O10 Cr1 O11 96.11(16) 7_566 . ?
O10 Cr1 O11 83.89(16) . . ?
O12 Cr1 O11 85.21(17) . . ?
O12 Cr1 O11 94.79(16) 7_566 . ?
O10 Cr1 O11 83.89(16) 7_566 7_566 ?
O10 Cr1 O11 96.11(16) . 7_566 ?
O12 Cr1 O11 94.79(16) . 7_566 ?
O12 Cr1 O11 85.21(17) 7_566 7_566 ?
O11 Cr1 O11 179.999(1) . 7_566 ?
O1 Mo2 O2 105.9(2) . . ?
O1 Mo2 O9 96.9(2) . . ?
O2 Mo2 O9 101.6(2) . . ?
O1 Mo2 O3 100.8(2) . . ?
O2 Mo2 O3 96.6(2) . . ?
O9 Mo2 O3 150.07(17) . . ?
O1 Mo2 O10 160.20(19) . . ?
O2 Mo2 O10 92.53(18) . . ?
O9 Mo2 O10 72.01(16) . . ?
O3 Mo2 O10 83.66(16) . . ?
O1 Mo2 O11 92.16(19) . . ?
O2 Mo2 O11 160.00(19) . . ?
O9 Mo2 O11 84.25(16) . . ?
O3 Mo2 O11 71.21(15) . . ?
O10 Mo2 O11 70.86(14) . . ?
O7 Mo3 O8 106.6(2) . . ?
O7 Mo3 O6 101.7(2) . . ?
O8 Mo3 O6 95.19(19) . . ?
O7 Mo3 O9 95.5(2) . 7_566 ?
O8 Mo3 O9 102.13(19) . 7_566 ?
O6 Mo3 O9 150.94(18) . 7_566 ?
O7 Mo3 O12 90.17(19) . . ?
O8 Mo3 O12 161.37(18) . . ?
O6 Mo3 O12 73.01(16) . . ?
O9 Mo3 O12 83.80(16) 7_566 . ?
O7 Mo3 O10 158.08(19) . 7_566 ?
O8 Mo3 O10 93.61(18) . 7_566 ?
O6 Mo3 O10 84.35(16) . 7_566 ?
O9 Mo3 O10 71.54(16) 7_566 7_566 ?
O12 Mo3 O10 71.30(14) . 7_566 ?
O5 Mo4 O4 106.4(2) . . ?
O5 Mo4 O6 101.0(2) . . ?
O4 Mo4 O6 97.9(2) . . ?
O5 Mo4 O3 97.2(2) . . ?
O4 Mo4 O3 100.2(2) . . ?
O6 Mo4 O3 149.43(17) . . ?
O5 Mo4 O11 159.5(2) . . ?
O4 Mo4 O11 92.6(2) . . ?
O6 Mo4 O11 83.39(16) . . ?
O3 Mo4 O11 71.45(15) . . ?
O5 Mo4 O12 90.9(2) . . ?
O4 Mo4 O12 161.4(2) . . ?
O6 Mo4 O12 71.41(15) . . ?
O3 Mo4 O12 84.03(16) . . ?
O11 Mo4 O12 71.42(14) . . ?
C4 N1 C5 123.3(6) . . ?
C4 N1 H1 118.3 . . ?
C5 N1 H1 118.3 . . ?
Mo2 O3 Mo4 119.1(2) . . ?
Mo3 O6 Mo4 118.2(2) . . ?
Mo3 O8 Tb1 156.6(2) . . ?
Mo2 O9 Mo3 118.4(2) . 7_566 ?
Cr1 O10 Mo3 102.67(16) . 7_566 ?
Cr1 O10 Mo2 103.64(16) . . ?
Mo3 O10 Mo2 93.65(14) 7_566 . ?
Cr1 O11 Mo4 102.19(17) . . ?
Cr1 O11 Mo2 101.61(16) . . ?
Mo4 O11 Mo2 94.09(14) . . ?
Cr1 O12 Mo3 102.56(16) . . ?
Cr1 O12 Mo4 101.17(16) . . ?
Mo3 O12 Mo4 92.96(14) . . ?
O8 Tb1 O8 77.6(2) . 2_656 ?
O8 Tb1 O14 81.29(16) . . ?
O8 Tb1 O14 74.09(15) 2_656 . ?
O8 Tb1 O15 141.57(16) . . ?
O8 Tb1 O15 71.36(15) 2_656 . ?
O14 Tb1 O15 110.49(18) . . ?
O8 Tb1 O14 74.09(15) . 2_656 ?
O8 Tb1 O14 81.29(16) 2_656 2_656 ?
O14 Tb1 O14 148.3(2) . 2_656 ?
O15 Tb1 O14 79.19(18) . 2_656 ?
O8 Tb1 O15 71.36(15) . 2_656 ?
O8 Tb1 O15 141.57(16) 2_656 2_656 ?
O14 Tb1 O15 79.19(18) . 2_656 ?
O15 Tb1 O15 145.4(2) . 2_656 ?
O14 Tb1 O15 110.49(18) 2_656 2_656 ?
O8 Tb1 O13 141.27(17) . . ?
O8 Tb1 O13 119.11(18) 2_656 . ?
O14 Tb1 O13 71.86(18) . . ?
O15 Tb1 O13 75.51(18) . . ?
O14 Tb1 O13 139.05(17) 2_656 . ?
O15 Tb1 O13 76.49(18) 2_656 . ?
O8 Tb1 O13 119.10(18) . 2_656 ?
O8 Tb1 O13 141.27(17) 2_656 2_656 ?
O14 Tb1 O13 139.06(18) . 2_656 ?
O15 Tb1 O13 76.48(18) . 2_656 ?
O14 Tb1 O13 71.86(18) 2_656 2_656 ?
O15 Tb1 O13 75.51(18) 2_656 2_656 ?
O13 Tb1 O13 71.3(3) . 2_656 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O17 C1 C2 C3 -158.0(8) . . . . ?
O16 C1 C2 C3 21.6(11) . . . . ?
O17 C1 C2 C6 21.1(10) . . . . ?
O16 C1 C2 C6 -159.3(7) . . . . ?
C6 C2 C3 C4 0.6(12) . . . . ?
C1 C2 C3 C4 179.6(8) . . . . ?
C2 C3 C4 N1 -0.6(13) . . . . ?
N1 C5 C6 C2 0.6(11) . . . . ?
C3 C2 C6 C5 -0.6(11) . . . . ?
C1 C2 C6 C5 -179.7(7) . . . . ?
C3 C4 N1 C5 0.6(13) . . . . ?
C6 C5 N1 C4 -0.6(12) . . . . ?
O1 Mo2 O3 Mo4 -70.4(3) . . . . ?
O2 Mo2 O3 Mo4 -178.1(2) . . . . ?
O9 Mo2 O3 Mo4 54.7(4) . . . . ?
O10 Mo2 O3 Mo4 90.1(2) . . . . ?
O11 Mo2 O3 Mo4 18.2(2) . . . . ?
O5 Mo4 O3 Mo2 179.2(3) . . . . ?
O4 Mo4 O3 Mo2 71.0(3) . . . . ?
O6 Mo4 O3 Mo2 -54.5(4) . . . . ?
O11 Mo4 O3 Mo2 -18.3(2) . . . . ?
O12 Mo4 O3 Mo2 -90.7(2) . . . . ?
O7 Mo3 O6 Mo4 -67.6(3) . . . . ?
O8 Mo3 O6 Mo4 -175.8(3) . . . . ?
O9 Mo3 O6 Mo4 57.5(5) 7_566 . . . ?
O12 Mo3 O6 Mo4 18.9(2) . . . . ?
O10 Mo3 O6 Mo4 91.1(2) 7_566 . . . ?
O5 Mo4 O6 Mo3 68.6(3) . . . . ?
O4 Mo4 O6 Mo3 177.1(3) . . . . ?
O3 Mo4 O6 Mo3 -56.9(5) . . . . ?
O11 Mo4 O6 Mo3 -91.2(2) . . . . ?
O12 Mo4 O6 Mo3 -18.6(2) . . . . ?
O7 Mo3 O8 Tb1 -91.1(7) . . . . ?
O6 Mo3 O8 Tb1 12.8(7) . . . . ?
O9 Mo3 O8 Tb1 169.4(6) 7_566 . . . ?
O12 Mo3 O8 Tb1 62.4(10) . . . . ?
O10 Mo3 O8 Tb1 97.5(6) 7_566 . . . ?
O1 Mo2 O9 Mo3 -178.1(3) . . . 7_566 ?
O2 Mo2 O9 Mo3 -70.2(3) . . . 7_566 ?
O3 Mo2 O9 Mo3 55.9(4) . . . 7_566 ?
O10 Mo2 O9 Mo3 18.7(2) . . . 7_566 ?
O11 Mo2 O9 Mo3 90.5(2) . . . 7_566 ?
O12 Cr1 O10 Mo3 -178.45(16) . . . 7_566 ?
O12 Cr1 O10 Mo3 1.55(16) 7_566 . . 7_566 ?
O11 Cr1 O10 Mo3 97.12(17) . . . 7_566 ?
O11 Cr1 O10 Mo3 -82.88(17) 7_566 . . 7_566 ?
O12 Cr1 O10 Mo2 84.56(17) . . . . ?
O12 Cr1 O10 Mo2 -95.44(17) 7_566 . . . ?
O11 Cr1 O10 Mo2 0.12(16) . . . . ?
O11 Cr1 O10 Mo2 -179.88(16) 7_566 . . . ?
O1 Mo2 O10 Cr1 32.1(6) . . . . ?
O2 Mo2 O10 Cr1 -168.7(2) . . . . ?
O9 Mo2 O10 Cr1 90.0(2) . . . . ?
O3 Mo2 O10 Cr1 -72.38(18) . . . . ?
O11 Mo2 O10 Cr1 -0.11(15) . . . . ?
O1 Mo2 O10 Mo3 -71.9(6) . . . 7_566 ?
O2 Mo2 O10 Mo3 87.30(19) . . . 7_566 ?
O9 Mo2 O10 Mo3 -14.03(15) . . . 7_566 ?
O3 Mo2 O10 Mo3 -176.37(16) . . . 7_566 ?
O11 Mo2 O10 Mo3 -104.09(16) . . . 7_566 ?
O10 Cr1 O11 Mo4 -83.30(17) 7_566 . . . ?
O10 Cr1 O11 Mo4 96.70(17) . . . . ?
O12 Cr1 O11 Mo4 -0.45(16) . . . . ?
O12 Cr1 O11 Mo4 179.55(16) 7_566 . . . ?
O10 Cr1 O11 Mo2 179.88(16) 7_566 . . . ?
O10 Cr1 O11 Mo2 -0.12(16) . . . . ?
O12 Cr1 O11 Mo2 -97.27(17) . . . . ?
O12 Cr1 O11 Mo2 82.73(17) 7_566 . . . ?
O11 Cr1 O11 Mo2 -80(31) 7_566 . . . ?
O5 Mo4 O11 Cr1 -30.8(6) . . . . ?
O4 Mo4 O11 Cr1 170.6(2) . . . . ?
O6 Mo4 O11 Cr1 72.97(18) . . . . ?
O3 Mo4 O11 Cr1 -89.43(19) . . . . ?
O12 Mo4 O11 Cr1 0.40(14) . . . . ?
O5 Mo4 O11 Mo2 72.0(6) . . . . ?
O4 Mo4 O11 Mo2 -86.5(2) . . . . ?
O6 Mo4 O11 Mo2 175.78(16) . . . . ?
O3 Mo4 O11 Mo2 13.38(15) . . . . ?
O12 Mo4 O11 Mo2 103.22(16) . . . . ?
O1 Mo2 O11 Cr1 -169.5(2) . . . . ?
O2 Mo2 O11 Cr1 35.3(6) . . . . ?
O9 Mo2 O11 Cr1 -72.81(18) . . . . ?
O3 Mo2 O11 Cr1 89.80(19) . . . . ?
O10 Mo2 O11 Cr1 0.11(15) . . . . ?
O1 Mo2 O11 Mo4 87.2(2) . . . . ?
O2 Mo2 O11 Mo4 -68.0(6) . . . . ?
O9 Mo2 O11 Mo4 -176.16(17) . . . . ?
O3 Mo2 O11 Mo4 -13.55(15) . . . . ?
O10 Mo2 O11 Mo4 -103.24(16) . . . . ?
O10 Cr1 O12 Mo3 1.55(16) 7_566 . . . ?
O10 Cr1 O12 Mo3 -178.45(16) . . . . ?
O12 Cr1 O12 Mo3 179(6) 7_566 . . . ?
O11 Cr1 O12 Mo3 -95.18(17) . . . . ?
O11 Cr1 O12 Mo3 84.82(17) 7_566 . . . ?
O10 Cr1 O12 Mo4 97.17(17) 7_566 . . . ?
O10 Cr1 O12 Mo4 -82.83(17) . . . . ?
O12 Cr1 O12 Mo4 -85(5) 7_566 . . . ?
O11 Cr1 O12 Mo4 0.44(16) . . . . ?
O11 Cr1 O12 Mo4 -179.56(16) 7_566 . . . ?
O7 Mo3 O12 Cr1 -169.5(2) . . . . ?
O8 Mo3 O12 Cr1 35.9(6) . . . . ?
O6 Mo3 O12 Cr1 88.3(2) . . . . ?
O9 Mo3 O12 Cr1 -74.00(18) 7_566 . . . ?
O10 Mo3 O12 Cr1 -1.43(14) 7_566 . . . ?
O7 Mo3 O12 Mo4 88.4(2) . . . . ?
O8 Mo3 O12 Mo4 -66.3(6) . . . . ?
O6 Mo3 O12 Mo4 -13.87(15) . . . . ?
O9 Mo3 O12 Mo4 -176.14(16) 7_566 . . . ?
O10 Mo3 O12 Mo4 -103.57(15) 7_566 . . . ?
O5 Mo4 O12 Cr1 169.1(2) . . . . ?
O4 Mo4 O12 Cr1 -32.4(7) . . . . ?
O6 Mo4 O12 Cr1 -89.5(2) . . . . ?
O3 Mo4 O12 Cr1 72.00(18) . . . . ?
O11 Mo4 O12 Cr1 -0.40(14) . . . . ?
O5 Mo4 O12 Mo3 -87.4(2) . . . . ?
O4 Mo4 O12 Mo3 71.0(6) . . . . ?
O6 Mo4 O12 Mo3 13.90(15) . . . . ?
O3 Mo4 O12 Mo3 175.43(16) . . . . ?
O11 Mo4 O12 Mo3 103.03(15) . . . . ?
Mo3 O8 Tb1 O8 66.2(6) . . . 2_656 ?
Mo3 O8 Tb1 O14 141.7(7) . . . . ?
Mo3 O8 Tb1 O15 29.5(8) . . . . ?
Mo3 O8 Tb1 O14 -18.2(6) . . . 2_656 ?
Mo3 O8 Tb1 O15 -136.9(7) . . . 2_656 ?
Mo3 O8 Tb1 O13 -172.3(5) . . . . ?
Mo3 O8 Tb1 O13 -76.2(7) . . . 2_656 ?

_diffrn_measured_fraction_theta_max 0.998
_diffrn_reflns_theta_full        25.00
_diffrn_measured_fraction_theta_full 0.998
_refine_diff_density_max         1.339
_refine_diff_density_min         -0.757
_refine_diff_density_rms         0.259
_database_code_depnum_ccdc_archive 'CCDC 940074'
#######################################################################
#
#                 Cambridge Crystallographic Data Centre
#                                CCDC 
# 
#######################################################################
# 
#  This CIF contains data from an original supplementary publication
#  deposited with the CCDC, and may include chemical, crystal,
#  experimental, refinement, atomic coordinates,
#  anisotropic displacement parameters and molecular geometry data,
#  as required by the journal to which it was submitted.
#
#  This CIF is provided on the understanding that it is used for bona
#  fide research purposes only. It may contain copyright material
#  of the CCDC or of third parties, and may not be copied or further
#  disseminated in any form, whether machine-readable or not,
#  except for the purpose of generating routine backup copies
#  on your local computer system.
# 
#  For further information on the CCDC, data deposition and
#  data retrieval see:
#                         www.ccdc.cam.ac.uk
#
#  Bona fide researchers may freely download Mercury and enCIFer
#  from this site to visualise CIF-encoded structures and 
#  to carry out CIF format checking respectively.
#
data_5

_audit_creation_method           'SHELXTL-NT2000 ver.6.12'
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'Cr Mo6 O30 Sm, 2(C6 H5 N O2), 4(O)'
_chemical_formula_sum            'C12 H10 Cr Mo6 N2 O38 Sm'
_chemical_formula_weight         1568.22

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cr Cr 0.3209 0.6236 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sm Sm -0.1638 3.4418 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Monoclinic
_symmetry_space_group_name_H-M   C2/c
_symmetry_space_group_name_Hall  '-C 2yc'

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'

_cell_length_a                   18.4316(14)
_cell_length_b                   12.5601(10)
_cell_length_c                   17.9491(14)
_cell_angle_alpha                90.00
_cell_angle_beta                 104.3000(10)
_cell_angle_gamma                90.00
_cell_volume                     4026.5(5)
_cell_formula_units_Z            4
_cell_measurement_temperature    298(2)
_cell_measurement_reflns_used    3470
_cell_measurement_theta_min      2.34
_cell_measurement_theta_max      28.02

_exptl_crystal_description       block
_exptl_crystal_colour            pink
_exptl_crystal_size_max          0.51
_exptl_crystal_size_mid          0.49
_exptl_crystal_size_min          0.45
_exptl_crystal_density_meas      2.507
_exptl_crystal_density_diffrn    2.587
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             2952.0
_exptl_absorpt_coefficient_mu    3.616
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.182
_exptl_absorpt_correction_T_max  0.196
_exptl_absorpt_process_details   '(SADABS; Bruker, 2000)'

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      298(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            8138
_diffrn_reflns_av_R_equivalents  0.0263
_diffrn_reflns_av_sigmaI/netI    0.0365
_diffrn_reflns_limit_h_min       -21
_diffrn_reflns_limit_h_max       21
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_theta_min         1.98
_diffrn_reflns_theta_max         25.00
_reflns_number_total             3547
_reflns_number_gt                3167
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0369P)²+26.4816P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         3533
_refine_ls_number_parameters     273
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0376
_refine_ls_R_factor_gt           0.0323
_refine_ls_wR_factor_ref         0.0810
_refine_ls_wR_factor_gt          0.0785
_refine_ls_goodness_of_fit_ref   1.040
_refine_ls_restrained_S_all      1.040
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
C1 C 0.3407(4) 0.4505(5) 0.4725(4) 0.0379(15) Uani 1 1 d . . .
C2 C 0.3462(3) 0.3331(5) 0.4548(4) 0.0314(14) Uani 1 1 d . . .
C3 C 0.3428(4) 0.2598(5) 0.5111(4) 0.0394(16) Uani 1 1 d . . .
H3 H 0.3373 0.2826 0.5587 0.047 Uiso 1 1 calc R . .
C4 C 0.3476(4) 0.1533(5) 0.4964(4) 0.0387(16) Uani 1 1 d . . .
H4 H 0.3453 0.1030 0.5339 0.046 Uiso 1 1 calc R . .
C5 C 0.3592(5) 0.1895(5) 0.3725(4) 0.0470(19) Uani 1 1 d . . .
H5 H 0.3651 0.1637 0.3258 0.056 Uiso 1 1 calc R . .
C6 C 0.3543(4) 0.2974(5) 0.3836(4) 0.0444(18) Uani 1 1 d . . .
H6 H 0.3563 0.3454 0.3447 0.053 Uiso 1 1 calc R . .
Cr1 Cr 0.2500 0.2500 0.0000 0.0180(3) Uani 1 2 d S . .
Mo1 Mo 0.38078(3) 0.26312(4) 0.16327(3) 0.02187(13) Uani 1 1 d . . .
Mo2 Mo 0.20901(3) 0.34026(4) 0.15920(3) 0.02161(13) Uani 1 1 d . . .
Mo3 Mo 0.42421(3) 0.17322(4) 0.00627(3) 0.02370(14) Uani 1 1 d . . .
N1 N 0.3556(3) 0.1227(4) 0.4281(3) 0.0337(12) Uani 1 1 d . . .
H1 H 0.3586 0.0556 0.4196 0.040 Uiso 1 1 calc R . .
O1 O 0.4257(2) 0.1578(3) 0.2125(3) 0.0366(10) Uani 1 1 d . . .
O2 O 0.4173(2) 0.3763(3) 0.2152(2) 0.0307(9) Uani 1 1 d . . .
O3 O 0.2893(2) 0.2420(3) 0.1950(2) 0.0252(9) Uani 1 1 d . . .
O4 O 0.2434(2) 0.4528(3) 0.2097(2) 0.0316(9) Uani 1 1 d . . .
O5 O 0.1487(2) 0.2859(3) 0.2067(2) 0.0342(10) Uani 1 1 d . . .
O6 O 0.1396(2) 0.4110(3) 0.0751(2) 0.0239(9) Uani 1 1 d . . .
O7 O 0.4849(2) 0.2266(4) -0.0415(3) 0.0372(11) Uani 1 1 d . . .
O8 O 0.4703(2) 0.0690(4) 0.0580(3) 0.0392(11) Uani 1 1 d . . .
O9 O 0.4339(2) 0.2819(3) 0.0845(2) 0.0275(9) Uani 1 1 d . . .
O10 O 0.3262(2) 0.1551(3) 0.0644(2) 0.0212(8) Uani 1 1 d . . .
O11 O 0.2886(2) 0.3547(3) 0.0818(2) 0.0206(8) Uani 1 1 d . . .
O12 O 0.17301(19) 0.2228(3) 0.0571(2) 0.0205(8) Uani 1 1 d . . .
O13 O 0.5091(3) 0.4732(3) 0.1225(3) 0.0371(11) Uani 1 1 d . . .
O14 O 0.6269(2) 0.5826(4) 0.2548(3) 0.0448(12) Uani 1 1 d . . .
O15 O 0.4825(3) 0.6850(4) 0.1690(3) 0.0482(13) Uani 1 1 d . . .
O16 O 0.3659(3) 0.5172(3) 0.4320(3) 0.0448(12) Uani 1 1 d . . .
O17 O 0.3103(3) 0.4700(4) 0.5253(3) 0.0592(15) Uani 1 1 d . . .
O1W O 0.1919(4) 0.4743(4) 0.3548(3) 0.0662(16) Uani 1 1 d . . .
O2W O 0.0394(6) 0.4088(9) 0.3236(4) 0.156(5) Uani 1 1 d . . .
Sm1 Sm 0.5000 0.52608(3) 0.2500 0.02271(12) Uani 1 2 d S . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
C1 O17 1.240(8) . ?
C1 O16 1.269(8) . ?
C1 C2 1.517(9) . ?
C2 C3 1.380(9) . ?
C2 C6 1.396(9) . ?
C3 C4 1.371(9) . ?
C3 H3 0.9300 . ?
C4 N1 1.328(8) . ?
C4 H4 0.9300 . ?
C5 N1 1.317(8) . ?
C5 C6 1.377(9) . ?
C5 H5 0.9300 . ?
C6 H6 0.9300 . ?
Cr1 O11 1.969(4) . ?
Cr1 O11 1.969(4) 7 ?
Cr1 O12 1.974(3) . ?
Cr1 O12 1.974(3) 7 ?
Cr1 O10 1.981(4) . ?
Cr1 O10 1.981(4) 7 ?
Mo1 O1 1.689(4) . ?
Mo1 O2 1.742(4) . ?
Mo1 O3 1.926(4) . ?
Mo1 O9 1.923(4) . ?
Mo1 O11 2.262(4) . ?
Mo1 O10 2.263(4) . ?
Mo2 O5 1.702(4) . ?
Mo2 O4 1.714(4) . ?
Mo2 O3 1.913(4) . ?
Mo2 O6 1.937(4) . ?
Mo2 O11 2.263(4) . ?
Mo2 O12 2.319(4) . ?
Mo3 O7 1.705(4) . ?
Mo3 O8 1.706(4) . ?
Mo3 O9 1.934(4) . ?
Mo3 O6 1.945(4) 7 ?
Mo3 O12 2.281(4) 7 ?
Mo3 O10 2.309(4) . ?
N1 H1 0.8600 . ?
O2 Sm1 2.405(4) . ?
O6 Mo3 1.945(4) 7 ?
O12 Mo3 2.281(4) 7 ?
O13 Sm1 2.428(4) . ?
O14 Sm1 2.425(4) . ?
O15 Sm1 2.444(4) . ?
Sm1 O2 2.405(4) 2_655 ?
Sm1 O14 2.425(4) 2_655 ?
Sm1 O13 2.428(4) 2_655 ?
Sm1 O15 2.444(4) 2_655 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O17 C1 O16 127.2(6) . . ?
O17 C1 C2 114.8(6) . . ?
O16 C1 C2 118.0(6) . . ?
C3 C2 C6 119.4(6) . . ?
C3 C2 C1 118.5(6) . . ?
C6 C2 C1 122.1(6) . . ?
C4 C3 C2 119.5(6) . . ?
C4 C3 H3 120.2 . . ?
C2 C3 H3 120.2 . . ?
N1 C4 C3 119.2(6) . . ?
N1 C4 H4 120.4 . . ?
C3 C4 H4 120.4 . . ?
N1 C5 C6 120.0(6) . . ?
N1 C5 H5 120.0 . . ?
C6 C5 H5 120.0 . . ?
C5 C6 C2 118.3(6) . . ?
C5 C6 H6 120.9 . . ?
C2 C6 H6 120.9 . . ?
O11 Cr1 O11 180.0(2) . 7 ?
O11 Cr1 O12 84.39(15) . . ?
O11 Cr1 O12 95.61(15) 7 . ?
O11 Cr1 O12 95.61(15) . 7 ?
O11 Cr1 O12 84.39(15) 7 7 ?
O12 Cr1 O12 180.0(3) . 7 ?
O11 Cr1 O10 83.86(15) . . ?
O11 Cr1 O10 96.14(15) 7 . ?
O12 Cr1 O10 95.19(15) . . ?
O12 Cr1 O10 84.81(15) 7 . ?
O11 Cr1 O10 96.14(15) . 7 ?
O11 Cr1 O10 83.86(15) 7 7 ?
O12 Cr1 O10 84.81(15) . 7 ?
O12 Cr1 O10 95.19(15) 7 7 ?
O10 Cr1 O10 180.0(2) . 7 ?
O1 Mo1 O2 106.5(2) . . ?
O1 Mo1 O3 95.13(19) . . ?
O2 Mo1 O3 101.80(17) . . ?
O1 Mo1 O9 101.95(19) . . ?
O2 Mo1 O9 95.40(17) . . ?
O3 Mo1 O9 151.19(16) . . ?
O1 Mo1 O11 158.23(17) . . ?
O2 Mo1 O11 93.46(17) . . ?
O3 Mo1 O11 71.89(14) . . ?
O9 Mo1 O11 84.27(15) . . ?
O1 Mo1 O10 90.37(18) . . ?
O2 Mo1 O10 161.32(17) . . ?
O3 Mo1 O10 84.14(15) . . ?
O9 Mo1 O10 72.84(14) . . ?
O11 Mo1 O10 71.36(13) . . ?
O5 Mo2 O4 105.6(2) . . ?
O5 Mo2 O3 96.91(18) . . ?
O4 Mo2 O3 101.52(18) . . ?
O5 Mo2 O6 100.77(18) . . ?
O4 Mo2 O6 96.93(18) . . ?
O3 Mo2 O6 149.92(16) . . ?
O5 Mo2 O11 160.44(17) . . ?
O4 Mo2 O11 92.68(16) . . ?
O3 Mo2 O11 72.10(14) . . ?
O6 Mo2 O11 83.58(14) . . ?
O5 Mo2 O12 92.64(17) . . ?
O4 Mo2 O12 159.86(17) . . ?
O3 Mo2 O12 84.38(15) . . ?
O6 Mo2 O12 70.75(14) . . ?
O11 Mo2 O12 70.61(13) . . ?
O7 Mo3 O8 106.0(2) . . ?
O7 Mo3 O9 97.63(19) . . ?
O8 Mo3 O9 101.6(2) . . ?
O7 Mo3 O6 100.76(18) . 7 ?
O8 Mo3 O6 96.85(19) . 7 ?
O9 Mo3 O6 149.15(16) . 7 ?
O7 Mo3 O12 93.23(18) . 7 ?
O8 Mo3 O12 159.29(18) . 7 ?
O9 Mo3 O12 83.02(15) . 7 ?
O6 Mo3 O12 71.46(14) 7 7 ?
O7 Mo3 O10 161.59(18) . . ?
O8 Mo3 O10 91.07(18) . . ?
O9 Mo3 O10 71.59(14) . . ?
O6 Mo3 O10 83.67(14) 7 . ?
O12 Mo3 O10 71.06(13) 7 . ?
C5 N1 C4 123.6(6) . . ?
C5 N1 H1 118.2 . . ?
C4 N1 H1 118.2 . . ?
Mo1 O2 Sm1 156.0(2) . . ?
Mo2 O3 Mo1 118.21(19) . . ?
Mo2 O6 Mo3 119.76(18) . 7 ?
Mo1 O9 Mo3 118.34(19) . . ?
Cr1 O10 Mo1 102.16(15) . . ?
Cr1 O10 Mo3 101.46(15) . . ?
Mo1 O10 Mo3 92.85(13) . . ?
Cr1 O11 Mo1 102.60(15) . . ?
Cr1 O11 Mo2 103.57(15) . . ?
Mo1 O11 Mo2 93.44(13) . . ?
Cr1 O12 Mo3 102.67(15) . 7 ?
Cr1 O12 Mo2 101.43(15) . . ?
Mo3 O12 Mo2 93.79(13) 7 . ?
O2 Sm1 O2 77.1(2) . 2_655 ?
O2 Sm1 O14 71.10(14) . 2_655 ?
O2 Sm1 O14 141.46(15) 2_655 2_655 ?
O2 Sm1 O14 141.46(15) . . ?
O2 Sm1 O14 71.10(14) 2_655 . ?
O14 Sm1 O14 145.9(2) 2_655 . ?
O2 Sm1 O13 81.00(15) . 2_655 ?
O2 Sm1 O13 74.25(14) 2_655 2_655 ?
O14 Sm1 O13 79.78(16) 2_655 2_655 ?
O14 Sm1 O13 109.73(17) . 2_655 ?
O2 Sm1 O13 74.25(14) . . ?
O2 Sm1 O13 81.00(15) 2_655 . ?
O14 Sm1 O13 109.73(17) 2_655 . ?
O14 Sm1 O13 79.78(16) . . ?
O13 Sm1 O13 148.3(2) 2_655 . ?
O2 Sm1 O15 140.84(15) . 2_655 ?
O2 Sm1 O15 120.18(16) 2_655 2_655 ?
O14 Sm1 O15 76.46(16) 2_655 2_655 ?
O14 Sm1 O15 75.85(16) . 2_655 ?
O13 Sm1 O15 72.08(16) 2_655 2_655 ?
O13 Sm1 O15 138.99(15) . 2_655 ?
O2 Sm1 O15 120.18(16) . . ?
O2 Sm1 O15 140.84(15) 2_655 . ?
O14 Sm1 O15 75.85(16) 2_655 . ?
O14 Sm1 O15 76.46(16) . . ?
O13 Sm1 O15 138.99(15) 2_655 . ?
O13 Sm1 O15 72.08(16) . . ?
O15 Sm1 O15 70.5(2) 2_655 . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O17 C1 C2 C3 -22.2(10) . . . . ?
O16 C1 C2 C3 159.0(6) . . . . ?
O17 C1 C2 C6 157.7(7) . . . . ?
O16 C1 C2 C6 -21.2(10) . . . . ?
C6 C2 C3 C4 0.2(11) . . . . ?
C1 C2 C3 C4 180.0(6) . . . . ?
C2 C3 C4 N1 0.1(11) . . . . ?
N1 C5 C6 C2 0.6(12) . . . . ?
C3 C2 C6 C5 -0.5(11) . . . . ?
C1 C2 C6 C5 179.7(7) . . . . ?
C6 C5 N1 C4 -0.3(11) . . . . ?
C3 C4 N1 C5 -0.1(11) . . . . ?
O1 Mo1 O2 Sm1 92.8(6) . . . . ?
O3 Mo1 O2 Sm1 -168.1(5) . . . . ?
O9 Mo1 O2 Sm1 -11.3(6) . . . . ?
O11 Mo1 O2 Sm1 -95.9(6) . . . . ?
O10 Mo1 O2 Sm1 -61.1(9) . . . . ?
O5 Mo2 O3 Mo1 -178.0(2) . . . . ?
O4 Mo2 O3 Mo1 -70.5(2) . . . . ?
O6 Mo2 O3 Mo1 56.2(4) . . . . ?
O11 Mo2 O3 Mo1 18.61(18) . . . . ?
O12 Mo2 O3 Mo1 90.0(2) . . . . ?
O1 Mo1 O3 Mo2 179.2(2) . . . . ?
O2 Mo1 O3 Mo2 71.2(3) . . . . ?
O9 Mo1 O3 Mo2 -54.3(4) . . . . ?
O11 Mo1 O3 Mo2 -18.64(18) . . . . ?
O10 Mo1 O3 Mo2 -90.9(2) . . . . ?
O5 Mo2 O6 Mo3 -70.6(2) . . . 7 ?
O4 Mo2 O6 Mo3 -177.9(2) . . . 7 ?
O3 Mo2 O6 Mo3 54.4(4) . . . 7 ?
O11 Mo2 O6 Mo3 90.1(2) . . . 7 ?
O12 Mo2 O6 Mo3 18.48(18) . . . 7 ?
O1 Mo1 O9 Mo3 67.8(3) . . . . ?
O2 Mo1 O9 Mo3 176.0(2) . . . . ?
O3 Mo1 O9 Mo3 -57.3(4) . . . . ?
O11 Mo1 O9 Mo3 -91.1(2) . . . . ?
O10 Mo1 O9 Mo3 -18.87(19) . . . . ?
O7 Mo3 O9 Mo1 -176.7(2) . . . . ?
O8 Mo3 O9 Mo1 -68.6(3) . . . . ?
O6 Mo3 O9 Mo1 57.0(4) 7 . . . ?
O12 Mo3 O9 Mo1 90.9(2) 7 . . . ?
O10 Mo3 O9 Mo1 18.61(19) . . . . ?
O11 Cr1 O10 Mo1 -1.20(14) . . . . ?
O11 Cr1 O10 Mo1 178.80(14) 7 . . . ?
O12 Cr1 O10 Mo1 -84.97(15) . . . . ?
O12 Cr1 O10 Mo1 95.03(15) 7 . . . ?
O10 Cr1 O10 Mo1 116(100) 7 . . . ?
O11 Cr1 O10 Mo3 -96.68(16) . . . . ?
O11 Cr1 O10 Mo3 83.32(16) 7 . . . ?
O12 Cr1 O10 Mo3 179.55(15) . . . . ?
O12 Cr1 O10 Mo3 -0.45(15) 7 . . . ?
O10 Cr1 O10 Mo3 20(100) 7 . . . ?
O1 Mo1 O10 Cr1 169.05(19) . . . . ?
O2 Mo1 O10 Cr1 -35.9(6) . . . . ?
O3 Mo1 O10 Cr1 73.93(17) . . . . ?
O9 Mo1 O10 Cr1 -88.55(18) . . . . ?
O11 Mo1 O10 Cr1 1.10(13) . . . . ?
O1 Mo1 O10 Mo3 -88.59(18) . . . . ?
O2 Mo1 O10 Mo3 66.5(5) . . . . ?
O3 Mo1 O10 Mo3 176.29(15) . . . . ?
O9 Mo1 O10 Mo3 13.81(14) . . . . ?
O11 Mo1 O10 Mo3 103.46(14) . . . . ?
O7 Mo3 O10 Cr1 33.0(6) . . . . ?
O8 Mo3 O10 Cr1 -168.9(2) . . . . ?
O9 Mo3 O10 Cr1 89.19(18) . . . . ?
O6 Mo3 O10 Cr1 -72.13(17) 7 . . . ?
O12 Mo3 O10 Cr1 0.41(13) 7 . . . ?
O7 Mo3 O10 Mo1 -70.0(6) . . . . ?
O8 Mo3 O10 Mo1 88.08(18) . . . . ?
O9 Mo3 O10 Mo1 -13.83(15) . . . . ?
O6 Mo3 O10 Mo1 -175.15(15) 7 . . . ?
O12 Mo3 O10 Mo1 -102.61(14) 7 . . . ?
O11 Cr1 O11 Mo1 -86(100) 7 . . . ?
O12 Cr1 O11 Mo1 97.06(16) . . . . ?
O12 Cr1 O11 Mo1 -82.94(16) 7 . . . ?
O10 Cr1 O11 Mo1 1.20(14) . . . . ?
O10 Cr1 O11 Mo1 -178.80(14) 7 . . . ?
O11 Cr1 O11 Mo2 177(100) 7 . . . ?
O12 Cr1 O11 Mo2 0.34(15) . . . . ?
O12 Cr1 O11 Mo2 -179.66(15) 7 . . . ?
O10 Cr1 O11 Mo2 -95.52(16) . . . . ?
O10 Cr1 O11 Mo2 84.48(16) 7 . . . ?
O1 Mo1 O11 Cr1 -35.4(5) . . . . ?
O2 Mo1 O11 Cr1 167.78(17) . . . . ?
O3 Mo1 O11 Cr1 -90.93(18) . . . . ?
O9 Mo1 O11 Cr1 72.69(17) . . . . ?
O10 Mo1 O11 Cr1 -1.10(13) . . . . ?
O1 Mo1 O11 Mo2 69.4(5) . . . . ?
O2 Mo1 O11 Mo2 -87.50(16) . . . . ?
O3 Mo1 O11 Mo2 13.80(14) . . . . ?
O9 Mo1 O11 Mo2 177.41(15) . . . . ?
O10 Mo1 O11 Mo2 103.62(14) . . . . ?
O5 Mo2 O11 Cr1 32.0(6) . . . . ?
O4 Mo2 O11 Cr1 -168.79(19) . . . . ?
O3 Mo2 O11 Cr1 89.96(18) . . . . ?
O6 Mo2 O11 Cr1 -72.11(17) . . . . ?
O12 Mo2 O11 Cr1 -0.30(14) . . . . ?
O5 Mo2 O11 Mo1 -71.8(5) . . . . ?
O4 Mo2 O11 Mo1 87.37(17) . . . . ?
O3 Mo2 O11 Mo1 -13.88(14) . . . . ?
O6 Mo2 O11 Mo1 -175.95(15) . . . . ?
O12 Mo2 O11 Mo1 -104.14(14) . . . . ?
O11 Cr1 O12 Mo3 96.25(16) . . . 7 ?
O11 Cr1 O12 Mo3 -83.75(16) 7 . . 7 ?
O12 Cr1 O12 Mo3 -108(100) 7 . . 7 ?
O10 Cr1 O12 Mo3 179.54(15) . . . 7 ?
O10 Cr1 O12 Mo3 -0.46(15) 7 . . 7 ?
O11 Cr1 O12 Mo2 -0.33(15) . . . . ?
O11 Cr1 O12 Mo2 179.67(15) 7 . . . ?
O12 Cr1 O12 Mo2 155(100) 7 . . . ?
O10 Cr1 O12 Mo2 82.96(16) . . . . ?
O10 Cr1 O12 Mo2 -97.04(16) 7 . . . ?
O5 Mo2 O12 Cr1 -169.37(19) . . . . ?
O4 Mo2 O12 Cr1 35.7(5) . . . . ?
O3 Mo2 O12 Cr1 -72.68(17) . . . . ?
O6 Mo2 O12 Cr1 90.14(17) . . . . ?
O11 Mo2 O12 Cr1 0.30(13) . . . . ?
O5 Mo2 O12 Mo3 86.88(18) . . . 7 ?
O4 Mo2 O12 Mo3 -68.1(5) . . . 7 ?
O3 Mo2 O12 Mo3 -176.43(15) . . . 7 ?
O6 Mo2 O12 Mo3 -13.61(13) . . . 7 ?
O11 Mo2 O12 Mo3 -103.45(14) . . . 7 ?
Mo1 O2 Sm1 O2 -66.4(5) . . . 2_655 ?
Mo1 O2 Sm1 O14 135.6(6) . . . 2_655 ?
Mo1 O2 Sm1 O14 -31.7(7) . . . . ?
Mo1 O2 Sm1 O13 -142.2(6) . . . 2_655 ?
Mo1 O2 Sm1 O13 17.8(6) . . . . ?
Mo1 O2 Sm1 O15 171.3(5) . . . 2_655 ?
Mo1 O2 Sm1 O15 75.5(6) . . . . ?

_diffrn_measured_fraction_theta_max 0.996
_diffrn_reflns_theta_full        25.00
_diffrn_measured_fraction_theta_full 0.996
_refine_diff_density_max         0.993
_refine_diff_density_min         -0.532
_refine_diff_density_rms         0.137
_database_code_depnum_ccdc_archive 'CCDC 946456'
